Multiscale constitutive model and computational
framework for the design of ultrahigh strength,
high toughness steels
Su Hao
a,b,
*
,Wing Kam Liu
b,
*
,Brian Moran
b
,Franck Vernerey
b
,
Gregory B.Olson
a
a
Department of Materials and Science Engineering,Northwestern University,2145 Sheridan Road,
Evanston,IL 602083111,USA
b
Department of Mechanical Engineering,The Technological Institute,Northwestern University,2145 Sheridan Road,Evanston,
IL 602083111,USA
Received 5 June 2003;received in revised form 16 October 2003;accepted 2 December 2003
Abstract
A multiscale hierarchical constitutive model is developed for establishing the relationship between quantum
mechanical,micromechanical,and overall strength/toughness properties in steel design.Focused on the design of ultra
high strength,high toughness steels,a twolevel cell model is used to represent two groups of hard particles (inclusions)
in an alloy matrix which is characteristic of such Febased alloys.Primary inclusion particles,which are greater than a
micron in size,are handled by a microcell.Secondary inclusion particles which are tens of nanometers in size are
modeled by a submicrocell.In the submicrocell,the matrix constitutive behavior is given by quantum mechanics
computation of bcciron calibrated according to experiments.In the microcell,the matrix constitutive behavior is given
by the stress–strain response of the submicrocell,characterized by a plastic ﬂow potential based on the numerical
simulation of the representative cell.In turn,the plastic ﬂow potential generated by the stress–strain response of the
microcell is used as the constitutive response at the continuummacro level for simulation of ductile fracture and for the
assessments of toughness.The interfacial debonding between the matrix and the primary and the secondary inclusion
particles are modeled using decohesion potentials computed through quantum mechanics calculation together with a
mechanical model of normal separation and gliding induced dislocation,which also provides quantitative explanations
why practice strength of a steel is much lower than the atomic separation force and how plasticity occurs in steels.
The ductile fracture simulations on an ASTMstandard center cracked specimen lead to the generation,for the ﬁrst
time,of a toughness,strength,adhesion diagram based on computer simulation and which establishes the relationship
between alloy matrix strength,interfacial decohesion energy,and fracture toughness.
2004 Elsevier B.V.All rights reserved.
Keywords:Multiscale multiphysics;Multiple scales;Plasticity;Constitutive law;Fracture toughness;Steel design;Materials design;
Particle dynamics;MD
*
Corresponding authors.Address:Department of Mechanical Engineering,The Technological Institute,Northwestern University,
2145 Sheridan Road,Evanston,IL 602083111,USA.Tel.:+8474917094;fax:+8474913915.
Email addresses:suhao@northwestern.edu,suhao1@yahoo.com(S.Hao),wliu@northwestern.edu (W.K.Liu),bmoran@north
western.edu (B.Moran),fvernerey@northwestern.edu (F.Vernerey),olson@igor.tech.northwestern.edu (G.B.Olson).
00457825/$  see front matter 2004 Elsevier B.V.All rights reserved.
doi:10.1016/j.cma.2003.12.026
Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
www.elsevier.com/locate/cma
1.Introduction
One of the principal objectives of micro/nanomechanics of materials is to account for the observed
phenomena and properties of macroscopic solid bodies,such as strength and fracture toughness of steels,
on the basis of the quantum mechanical theory of the behavior of atomic particles.Success will have been
achieved when it becomes possible to calculate the quantities that describe the constitution of materials and
their response to alterations of macroscopic mechanical boundary conditions from the knowledge of the
component elements and their hierarchical structures from atomistic–electronic scales to micro and
macroscales.This is particularly important for steel design.
For this purpose,the diﬃculties and complexity originate in the substantial diﬀerences in philosophy and
viewpoints between conventional continuummechanics and quantumtheory.In the former,the solution of
a boundary value problem is uniquely determined based on Newtons laws when initial and boundary
conditions are given;whereas the Heisenberg uncertainty principle,the cornerstone of quantummechanics,
indicates that motion of a particle is characterized by wave solutions of Sch
€
odingers equation and the
intensity of wave solutions deﬁnes the ‘‘probability density’’ for the position of this particle.For mechanical
engineers,the challenges lie in how to establish the relationship between a continuum mechanical system
and its atomistic–electronic structure and how to constitute a uniﬁed framework that bridges the mecha
nisms from diﬀerent scales.These are the keyissues in the ONR project ‘‘cybersteel2020’’ [1] towards the
predictive design of novel steels to combine high strength and fracture toughness.
Both strength and fracture toughness are the key propertyindices for steels.Although advanced tech
nology currently provides many ways to achieve either high strength or high toughness,respectively,in steel
through manufacturing processes,it remains a challenge to achieve both of them simultaneously.This is
because the toughness characterizes the capability of a material against fracture at a crack tip local.The
diﬀerence between the local and the global properties reﬂects the natural heterogeneity of the micro
structure of steels.The design of steels seeks to achieve desirable micro/nanostructures with optimized
properties through alloy component/phase selection and metallurgical processes based on quantitative
understanding of controlling mechanisms and the relationships among these at diﬀerent scales.
In this paper,a bottomup computational methodology has been proposed to establish a hierarchical
multiphysics constitutive model that builds up the relationships among the macroscale properties,micro
and submicrostructures,and atomistic failure modes for steels.To this end,new models and computa
tional schemes have been developed.The innovations presented here can be summarized as follows:
1.We propose an atomistic adhesion model that counts for both the separation normal to newly created
interfaces and gliding induced dislocations.The normal separation is described as a creation of empty
sites,which may trigger gliding induced dislocation that translates the shortranged covalent binding
force into a longranged decohesion law.Rices criterion [2] is used to determine these two competing
mechanisms.The computed results provide a quantitative explanation why the practical strength of a
steel is much lower than the prediction of atomic separation and how plasticity occurs in steel.
2.A ﬁrstprinciple based ab initio computation has been performed to calculate the generalized fault en
ergy against dislocation induced sliding in a bccFe crystal.
3.A‘‘Quasiparticle dynamics approach’’ has been developed,which transforms an atomistic systeminto a
‘‘particle system’’ while maintaining intrinsic structural properties such as crystal elastic constants and
molecular dynamic kinetics.Each particle can be a ‘‘superatom’’ containing several atoms,or represents
an inclusion particle,depending upon the scales of interest.As the particle systemcan have fewer degrees
of freedom than the atomistic system,the method can be used for bridging atomistic and continuum
scales.
4.A hierarchical multiphysics computational constitutive model has been developed based on a uniﬁed
thermodynamic framework.This model is applied in a computation procedure,which is named as a
1866 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
‘‘ductile fracture simulator’’ by the authors,to support quantitative tradeoﬀ analysis in microstructural
optimization for fracture toughness.
5.A toughness–strength–adhesion diagram has been obtained for steel design,which establishes the rela
tionship among alloy matrix strength,inclusion adhesion interfacial energy and fracture toughness.To
the authors knowledge this is the ﬁrst computer generated design diagram for engineering application.
This paper is organized as follows:In Section 2 we introduce the hierarchical model.Section 3 describes
the quantum physics analysis and the bridge to continuum mechanics.The Quasiparticle dynamics ap
proach is introduced in Section 4.A uniﬁed multiphysics thermodynamic framework in continuum
mechanics and a twolevel cell representation at submicro and microscales are derived in Section 5,which
lead to a hierarchical constitutive model.Simulations of crack propagation and fracture toughness are
presented in Section 6.As a conclusion,a toughness–strength–adhesion diagram is developed.This dia
gram,together with the hierarchical constitutive model and computational procedure,constitute the
‘‘ductile fracture simulator’’ presented in Section 7.
2.Methodology and approach
Like all conventional materials,steels are heterogeneous innature.A modern ultrahigh strength steel
generally consists of an alloy matrix with several levels of dispersed small hard inclusion particles (see Fig.
1).Interfacial strength between the diﬀerent phases plays an important role in the strength and toughness of
steels.
For the ultrahigh strength steels considered here,dispersions of hard particles occur at two distinct
scales:primary particles (such as TiN,MgS,Fe
3
C) are typically on the order of microns in size;and sec
ondary particles (such as TiC,TiC
2
S and M
2
C compounds) are on the order of tens of nanometers in size.
To develop a macroscopic constitutive model for ultrahigh strength,high toughness steel,we propose a
multiphysics approach based on hierarchical unit cell representations of the primary particles and sec
ondary particles.A quantum mechanical analysis is performed to determine the constitutive relations for
Fig.1.A TEM micrograph of the fracture surface of a ultrahighstrength steel (with the courtesy of Prof.G.Kruass,School of
Corolado of Mine).
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1867
the iron matrix and the interfacial behavior between the matrix and the inclusions,leading in turn to the
continuum mechanics decohesion potentials for diﬀerent interfaces and alloy matrices.A continuum
mechanics analysis is applied in the unit cell representation with primary particles,which we call
‘‘microscale cell model’’.A ‘‘Quasiparticle dynamics approach’’ is developed for the cell representation
with secondary particles,which is termed ‘‘submicrocell model’’.At the quantum scale,the subatomic
primitive cells are applied in interfacial separation and bulk iron matrix adhesion analyses.Thus,the
proposed approach links mechanisms from quantumatomistic scales and micro/submicroscales to the
scale of a laboratory fracture toughness specimen,as demonstrated in the ﬂow chart of Fig.2a and brieﬂy
illustrated in Fig.2b.
In Fig.2b and in the following analysis,r
ij
and e
ij
denote the stresses and strains at the submicroscale.
The submicroscale cell model homogenizes r
ij
and e
ij
into the microscale stress and strain which are de
noted by R
micro
ij
and E
micro
ij
,respectively;and a microscale plastic potential U
micro
is developed.By repeating
this procedure the macroscale stress–strain:R
ij
,E
ij
,and the corresponding macroscale plastic potential
U
macro
,are obtained,which is applied to the laboratory specimen to fracture simulation.
In the following section,we begin with a description of the crystal separation behavior and the
underlying quantum mechanical consideration,leading to a continuum mechanics force–separation law.
3.Interfacial separation:from quantum mechanics to continuum mechanics
3.1.Interfacial separation:from quantum nanomechanics to continuum micromechanics
For a metallic or intermetallic systemwhere each atomhas a suﬃcient number of electrons,the Thomas
Fermi [3,4] model is applicable.This model approximates the system as a combination of static atomic
cores that formthe crystal and an electronic gas that ﬁlls the space among the atoms.Hohenberg and Kohn
[5] and Kohn and Shams [6] theorems indicate that the groundstate energy of such a many body system,
which is an eigenvalue of the corresponding wave solution of the Schr
€
odinger equation,is determined by
electron density distribution.Based on the augmented plane wave method introduced by Slater [7],various
numerical methods have been developed to determine the electron density distribution,e.g.[8–11].Among
them,the fullpotential spinpolarized linear augmented plane wave (FLAPW) [12] is presently considered
to be the most accurate scheme as it holds the fewest approximations.
Macroscopic fracture of a crystal is a process whereby atomic aggregates are split into two parts.For a
defectfree system where separation is normal to the newly created surfaces,Rose et al.[13] found that the
binding energy obeys an approximate ‘‘universal relation’’ of the form
E
N
ðk
N
Þ ¼ ½Eðk
N0
Þ Eð1Þ E
N
k
N
l
TF
;
k
N0
l
TF
;ð3:1Þ
where E
N
ðk
N
Þ is the binding energy;k
N
is the normal separation and k
N0
is the normal separation at the
equilibrium state;Eðk
N0
Þ and Eð1Þ are the total groundstate energies of the system at k
N0
and k
N
!1,
respectively;l
TF
is a scaling length which characterizes an atomic size and E
N
is function which describes the
shape of E
N
ðk
N
Þ.When the system is fully separated and no extra strain is imposed before and after this
separation,the change of the total groundstate energy is identical to the newly created surface energy,i.e.
2Ac
F
¼ Eðk
N0
Þ Eð1Þ;ð3:2Þ
where c
F
is the surface energy per unit area and A is the area of the newly created surfaces.
Real crystals may contain a variety of imperfections,e.g.impurity or interstitial atoms,vacant lattice
site,and dislocations.The normal separation (3.1) can be viewed as the creation of new vacant lattice sites,
1868 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
Fig.2.(a) The ﬂow chart of the proposed approach.(b) An illustration of the proposed hierarchical model that links a:the quantum
scale,b:submicroscale,c:microscale,d:macroscale.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1869
which may trigger other defects,such as the motion of dislocations along interacting slip planes.Rices
criterion [2] states that dislocation motion will be activated when the energy barrier,c
US
,against unstable
sliding is smaller than the cleavage surface energy,c
F
,which provides a basis for describing the competition
between these two mechanisms.The mathematical expression of Rices criterion is:
c
F
c
US
j
R
> 1;ð3:3Þ
where j
R
is a function of the average lattice elastic stress and the angle/between the slipplane and the
newlycreated surface,and j
R
< 1.When dislocation induced sliding occurs,the relation between the total
system energy E
S
and sliding separation k
S
per dislocation can be written as:
E
S
ðk
S
Þ ¼ c
US
E
S
ðk
S
;/Þ;ð3:4Þ
where E
S
ðk
S
;/Þ is a normalized function which describes the shape of E
S
ðk
S
Þ.
Weertman [14] studied a rectangular wave shape for E
S
ðk
S
;/Þ.Based on the Peierls concept for a
monoclinic crystals,an approximate expression for E
S
is suggested in [2]
E
S
¼ sin
4
pk
S
b
:ð3:5Þ
The relations (3.1)–(3.4) are fundamental equations of atomistic fracture.To obtain accurate values of c
F
and c
US
,and expressions for E
S
and E
N
,ﬁrst principlebased calculations are required which will be
introduced in the next section.The quantum mechanics formulation and the method used to obtain these
quantities are brieﬂy described in Appendix A.
In this paper the ﬁrstprinciple calculations are used to compute the binding energy relations for the
following systems:
(1) iron matrix:normal adhesion and sliding;
(2) interfacial decohesion between alloy matrix and TiC
x
N
1x
particles (x ¼ 0:primary particle;x ¼ 1:sec
ondary particle).
3.2.Firstprinciple computations
The fundamentals of ﬁrstprinciple computation are introduced in [8,11,12] based on density functional
theory [5,6].
The most important step of a ﬁrstprinciple computation of a crystal is to set up the corresponding
geometrical model,i.e.the primitive cell of atomistic analysis.A density functional theory (DFT) based
computation requires the calculation of charge density distribution among atoms.It is crucial to design a
primitive cell that is able to represent the fundamental physics yet which contains suﬃciently small numbers
of atoms so as to be computationally treatable.
The starting point for designing an atomistic primitive cell in this study is presuming that the interested
atomic structures of iron and the Fe/TiC interface are much smaller than those geometrical parameters such
as particle/grain sizes,so that an iron crystal can be considered to be an inﬁnite slab of atoms and the Fe/
TiC interface can be considered to be the boundary between a semiinﬁnite iron slab and semiinﬁnite TiC
slab.Since interatomic forces (covalent binding forces) are shortrange in nature,it is reasonable to design a
repeatable subatomic cell with the minimumrequisite number of atoms by using the periodic structure of a
crystal.
In the following analysis,we use ‘‘AkB’’ to denote the interface between crystal A and B.For example,
‘‘f001g
Fe
bcc
kf001g
TiC
fcc
’’ denotes the interface between a {0 01} surface of a bccFe crystal and a {00 1}
surface of a (NaCl structured) fccTiC crystal,as shown in Fig.3a.
1870 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
For a system such as the Fe/TiC interface shown in Fig.3a,the following failure modes may occur:
1.normal and sliding separations in Fe;
2.normal and sliding separations in the TiC;
3.Fe/TiC interfacial debonding.
The TiC,as a ceramic,has a much higher coherent strength than Fe [15],so the failure mode 2 is ex
cluded in this analysis.
Both the normal separation and shear sliding in iron matrix have been studied in this paper.We have
computed the ½
1
11 shear fault energy on the ð1
11Þ plane,the normal separation of Fe–Ti site of the
f001g
Fe
bcc
kf001g
TiC
fcc
interface,and the separation normal to {11 1} plane in a perfect bccFe crystal with
twoempty sites using the linearized augmented plane wave code based on [9].These computations,in
conjunction with the results from collaborators [16,17] and the literature [15,18],provide a clear picture of
decohesion process of the steel at the quantum scale.The details are given as follows.
3.2.1.Normal separation
3.2.1.1.Fe–Ti site at TiC–bccFe interface.For the interface decohesion problem,the diﬃculty lies in the
anisotropicnature of crystalline structures and the misﬁt in lattice constants between the two diﬀerent
crystals.It is well known that at roomtemperature Fe exists as a bcc crystal with a lattice constant of 0.287
nm [19] and TiC exists as a NaCl(fcc) structure with a lattice constant 0.4332 nm [15,20] (Fig.3a).The
challenge is to ﬁnd the sites which have the minimum lattice misﬁt and the strongest binding energy,thus
which form the most coherent junctions among the combinations of Fe–TiC interfacial structures.
For bccFe,the distances from an atom to its most closest neighbors are 0.249 nm (between bcc corner
and center atoms),0.287 nm (the edge length of a cubic unit of bcc crystal),and 0.407 nm (between the
diagonal atoms pair on the surface of a cubic bcc unit).Obviously,the last one is the site with the minimum
misﬁt to the lattice constant (0.4332 nm) of the TiC.Hence,the f001g
Fe
bcc
kf001g
TiC
fcc
junction matches the
Fig.3.(a) Coherent TiC–Fe [1 00] interface;(b) topdown view ([0 0
1]) of the TiC/Fe interface with the neighbored Fe layer and TiC
layer where Fe atoms sit on the saddle point of TiC crystal.Fe–C site:the Fe crystal moves as indicated by the vector
a;Fe–Ti site:the
Fe crystal moves by the vector
b.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1871
most preferred binding surfaces of both sides with three possible arrangements:Fe–C site,Fe–Ti site,and
Fe–TiC saddle point site (see Fig.3b).
The study of the coherent Fe–TiC interface was ﬁrst performed by Freemans group [17] using FLAPW
[21].In this paper the simulation and calibration of (3.1) and (3.2) of the subatomic cell of
f001g
Fe
bcc
kf001g
TiC
fcc
decohesion is computed.The interfacial debonding energies are listed in Table 1.
It should be pointed out that the primitive model of Fig.3a actually represents the interface of a
periodically repeated Fe/TiC layered structure.The height of each layer is twice times of the atoms layers
plotted in the ﬁgure.In this primitive cell analysis the eﬀects of layer overlay are omitted.
3.2.1.2.Decohesion normal to (11 1) in bcciron.A subatomic cell is developed as illustrated in Fig.4a,
where the primitive vectors take the form
a ¼
^
x þ
^
y;
b ¼
^
y þ
^
z;
c ¼
^
x þ
^
y þ
^
z;ð3:6Þ
which are originated at ð
^
x;0;0Þ.Presuming the six outer surfaces of the cell to be rigid,periodic boundary
conditions are imposed on the two surfaces pairs:f0;y
b;z
cg and f
a;y
b;z
cg as well as fx
a;0;z
cg and
fx
a;
b;z
cg;where (x;y;z) are the coordinates deﬁned in the system f
a;
b;
cg.The surfaces fx
a;y
b;0g and
fx
a;y
b;
cg are enforced to move oppositely normal to the (1 11) plane.For the case with twoempty sites,
the two middle atoms marked with dark color inside are taken away.The subatomic cell is periodically
Table 1
Surface energies and equilibrium separations––results of ﬁrst principle calculations
Decohesion surface Interface 2c
F
(J/M
2
) k
N0
(nm) Source
f001g
Fe
bcc
kf001g
TiC
fcc
Fe–C site 3.82 0.213 [17]
f001g
Fe
bcc
kf001g
TiC
fcc
Fe–Ti site 0.61 0.361 This work (Fig.4b)
{11 1} Perfect 5.43 0.094 This work (Fig.4b)
{11 1} Perfect 5.38 0.0809 [18]
{11 1} Twoempty sites 1.1 0.241 This work (Fig.4b)
½
1
11 stacking fault Fe–Fe c
US
¼ 0:43 (J/M
2
) This work (Fig.6)
Fig.4.(a) Subatomic cell for {111} plane separation in bcciron crystal and (b) the computed energyseparation relations for three
cases.
1872 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
reproducible throughout space.The 12 ·12·1 kpoint mesh with Monkhorst and Pack scheme is applied in
the simulations.
3.2.1.3.Results of normal separation.The results are summarized in Table 1.The corresponding computed
energyseparation curves are plotted in Fig.4b.
3.2.2.Gliding induced dislocation
The stacking fault energy barrier c
US
is a crucial parameter for materials,as Eq.(3.3) indicates that the
ratio of
c
F
c
US
determines the mode of separation,which determines toughness.This is because at macroscale,
normal separation represents brittle fracture whereas atomistic sliding corresponding to plastic ﬂow.When
c
US
< c
F
,gliding induces dislocation motions.A dislocation core is an empty site that reduces the deco
hesion energy signiﬁcantly when normal decohesion occurs,see Fig.4b and Table 1.
There is a considerable amount of research on ﬁrst principlebased simulations of stacking fault
mechanisms in fcc crystal,e.g.[22],whereas few results are reported for Febcc crystals.In a bcc crystal,
sliding along {110} planes in the h111i direction is an often observed active screw dislocation pattern.
Because sliding may turn from one h111i direction to another,it usually moves along a zigzag path.A
½
1
11 fault is a possible composition of several zigzag motions.
In this paper,we study the ½
1
11 fault.The importance of this motion is that two such stacking faults
form a complete glide dislocation,i.e.:
a
2
½
1
11 þ
a
2
½111!a½001;ð3:7aÞ
where ‘‘a’’ is lattice constant.A ½
1
11 fault can be decomposed into the following three steps:
a
2
½
1
11!
a
8
½
1
10 þ
a
4
½
1
12 þ
a
8
½
1
10;ð3:7bÞ
which is formed by a zigzag path on the ð1
10Þ plane.It moves ﬁrst along the intersection of ð1
11Þ and
ð1
10Þ planes which is the line segment ½
1
10;then moves along the intersection of (1 11) and ð1
10Þ planes
which is the line segment ½
1
12 and ﬁnally back to the direction of line segment ½
1
10.In Fig.5,a primitive
cell representing the periodic repeating motion of (3.7b) is given.Its primitive vectors,which originate at
ð0;
^
y;
^
zÞ,take the form
a ¼
a
2
½
^
x
^
y þ
^
z;
b ¼
a
2
½
^
x þ
^
y þ
^
z;
c ¼
a
2
½ð1 qÞ
^
x ð1 qÞ
^
y gðqÞ
^
z;ð3:8Þ
Fig.5.The primitive cell for a [
1
11] dislocation.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1873
where q varies from 0 to 1,representing the gliding induced sliding;and
gðqÞ ¼
1 q < 0:25;
3 4q
2
0:256q < 0:75;
0 q P0:75:
8
>
>
<
>
>
:
The computed energysliding relation is plotted in Fig.6,which demonstrates the energy barrier c
US
for the
motion of
a
8
½
1
10 is about 0.31 J/M
2
and the c
US
for
a
4
½
1
12 is about 0.43 J/M
2
.
Recall Rices criterion (3.3)
c
F
c
US
j
R
ð/Þ > 1;
where j
R
ð/Þ 0:3.Comparing Fig.6 and the results listed in Table 1,we conclude that at the Fe–C site of
the TiC/Fe interface and in a perfect bccFe matrix,relation (3.3) is satisﬁed so that sliding induced
separations dominate the decohesion process.Under these situations,fracture is ‘‘intrinsically’’ ductile.
Also from Table 1 we ﬁnd that point defects,such as vacancies,have a strong eﬀect on the fracture
mechanisms since they reduce the decohesion energy signiﬁcantly,and thus transform a ductile fracture to
brittle.
3.2.3.The ‘‘c plane’’ sliding
According to the diﬀerence in decohesion energy between the Fe–C site and the Fe–Ti site (see Table 1),
we obtain an estimate of (3.4) for the sliding tangential to the Fe–TiC interface,termed ‘‘c plane’’ sliding:
E
c
ðk
c
Þ ¼ A
S
sin
4
pk
cx
b
sin
4
pk
cy
b
;ð3:9Þ
where
A
S
¼
k
Nc
0
k
N
6
ðc
S
j
Fe–C
c
S
j
Fe–Ti
Þ;
k
Nc0
¼ 0:213 nm,b is taken as the average of the lattice constants of TiC (0.4332 nm) and Fe (0.407 nm);k
cx
,
k
cy
are the projections of k
c
onto the x and yaxis in Fig.3b,respectively;when k
Sx
¼ k
Sy
¼ 0,it refers to the
Fe–C site.
Fig.6.The energydislocation core position curve of [
1
11] dislocation.
1874 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
3.3.A proposed potential approach based on Needleman’s potential and quantum mechanics simulation
Needleman [23] developed an interface cohesive model that deﬁnes the normal traction ðr
N
Þ and tan
gential traction ðr
T
Þ along the interface through a potential W
interface
r
N
¼
oW
interface
o½u
N
;r
T
¼
oW
interface
o½u
T
;ð3:10Þ
where ½u
N
,½u
T
are normal and tangential interfacial separations,respectively.An expression for U
i
is given
in [23] which is calibrated using experimental results [24].
In this study,we split the Needlemans potential into normal separation part W
N
and tangential part W
T
,
respectively
r
N
¼
oW
N
o½u
N
;r
T
¼
oW
T
o½u
T
:ð3:10aÞ
According to (3.1)–(3.4),we propose that the W
N
and W
T
take the forms of
W
N
¼ E
N
þj
slide
X
E
S
;W
T
¼ E
c
;ð3:11Þ
where E
N
is given in Table 1;E
c
is given by (3.9).
P
E
S
is the summation of sliding energy for all slip
systems except the c plane and j
slide
is a coeﬃcient to be determined;which will be discussed in the next
section.
3.4.Rescaling factor
The expression (3.11) is inconvenient for continuum mechanical analysis when no sliding occurs.This is
because (3.1) describes a process of covalent bond breaking which is very shortranged.The corresponding
force usually becomes negligible when separation is greater than 1 nm,which is not an appropriated scale
for continuummechanics.On the other hand,it is also not trivial to compute the term‘‘j
slide
P
E
S
’’ in (3.11)
accurately.
The previous analysis indicates that iron is ‘‘intrinsically ductile’’.When normal separation consorts with
a dislocation induced sliding,the shortranged force deﬁned by (3.1) may be transformed into a longer
range force.This mechanism is schematically illustrated in Fig.7.In this ﬁgure the separation of the
interface A is caused by the separation imposed on the two ends of the dashed box,which contains all
motions within the box.Fig.7a is the no sliding case where (3.3) is not satisﬁed;while Fig.7b shows the
case where k
N
is a combination of the normal components of gliding induced separations plus the normal
separation between interfacial atompairs.Dislocation motion may thus roughen a fracture surface and,
thereby modify the total surface energy and peak stress.
The mechanism proposed in Fig.7a and b can be stated as the following two hypotheses:
1.The tangential components of dislocation induced sliding trade oﬀ against each other,except the sliding
along the cplane.
2.If we assume that the change of surface energy is negligible,then the normal components of all sliding
induced separations reduce the peak separation force through rescaling the universal function E
N
.de
ﬁned in (3.1) in the following manner:
E
N
þj
slide
X
E
S
¼ 2c
F
E
N
j
k
N
k
N0
l
TF
;ð3:12Þ
where j is a rescaling parameter to be discussed in the following sections.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1875
By substituting (3.12) into (3.11),the latter becomes
W
N
¼ 2c
F
E
N
j
k
N
k
N0
l
TF
ð3:13Þ
and
W
T
¼ E
c
:ð3:14Þ
In this paper the eﬀect of dislocation induced atomic vibration (dislocation–phonon interaction) is
omitted.
Fig.7.Normal separation and sliding induced separation:(a) pure normal separation;(b) mixed separation–separation strength
weakens and (c) a dislocation induced sliding may cause a zigzag morphology at fracture surface.
1876 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
3.5.Grain boundary segregation
An Fe–TiC interface can be viewed as a grain boundary.This is because in practices it is nontrivial to
control all surfaces of a TiC particle to be perfectly coherent to alloy matrix.The vicinity of a grain
boundary interface can be represented by three regions:grain A,grain B,and an interfacial zone h;as
illustrated in Fig.8.Irregularities such as misﬁt in lattice constants,mismatch in atomistic properties and
crystal orientations,molar fraction of the solute,and the free volume in h,may change the energysepa
ration potentials (3.13) and (3.14) signiﬁcantly [25].
According to the thermodynamic description of interfacial segregation,e.g.[26–29],during a fast
fracture at low temperature the reduction of the ideal (Griﬃth) work of separation can be expressed by [27]:
2c
F
¼ 2c
0
F
l
X
I
l
X
S
C
X
;ð3:15Þ
where c
0
F
is the separation energy in a pure system without segregate elements,the superscript ‘‘X’’ denotes
the quantities associated with a segregate element X:C
X
is the quantity of the composition X per unit area
of interface,l
X
I
is the (interfacial) chemical potential of X before separation and l
X
S
is the chemical potential
of the bulk surface phase of X after separation.The value of the quantity ðl
X
I
l
X
S
Þ,where X is one among
the elements of Carbon (C),Phosphorus (P),Tin (Sn),Antimony (Sb),Sulfur (S),are given in [27] based on
experimental data.
Hence,when an interface structure is ﬁxed,the rescaling parameter j in (3.13) can be computed
accurately.However,it is impractical to do this case by case in engineering design.Accordingly,we
introduce an ad hoc estimate of j for our application.
The idealized coherent interface,e.g.that in Fig.3,can be considered as a degenerate case of Fig.8 when
h ¼ 0 and h ¼ a
i
,where a
i
is the interatomic distance at the interface and it has the same order as the lattice
constants of the matrices.An ad hoc estimate of the rescaling parameter j in (3.13) is
j ¼
a
i
h
:ð3:16Þ
Alber and Bassani [30] have performed a series of molecular dynamic simulation of the R3 and R5 grain
boundaries.According to the variation of the computed elastic constants their results suggest that h 5a
where a is the lattice constant of A and B in Fig.3 when A¼B.Accordingly,we use a value of j ¼ 1=5 in
this paper,which predicts the maximum separation stress of 6 GPa at the Fe–C site of f001g
Fe
bcc
kf001g
TiC
fcc
interface.This estimate matches experimental results for the commercial steel (modiﬁed 4340 steel) that will
be studied later.This steel shows that the maximum value of ﬂow stress,r
flow
,is near 2 GPa.The slipline
Fig.8.Schematic diagram of a grain boundary.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1877
analysis [23,24] indicates that the maximumseparation stress between a hard inclusion and an iron matrix is
approximately ð1 þ
ﬃﬃﬃ
3
p
Þr
flow
.
Finally,we obtained the normal tractionseparations for the Fe–TiC interface which are plotted in Fig.9
using j ¼ 1=5 to calibrate (3.13) based on the results in Fig.4b and Table 1.The curve with the maximum
peak stress is corresponding to the Fe–C site separation while the one with the lowest peak stress is cor
responding to the Fe–Ti site separation.
4.Quasiparticle dynamics approach
1
As mentioned in Section 2,the secondary particles in ultra high strength steel are on the order of tens
nanometers in size.Materials decohesion and fracture at this scale may depend strongly on atomistic
properties,such as crystal periodicity and orthogonal anisotropy.Molecular dynamics (MD) is an
appropriate method to bridge the quantum physics to continuum mechanical analysis at this scale.
The application of molecular dynamics is hampered by the computational demands of simulating a
suﬃciently large number of atoms to represent the physical phenomenon of interest.The interatomic
distances in a crystal are at the order of Angstroms.Hence,a simulation of a 3D cell model with the
dimension of hundreds nanometers requires about 10
9
atoms.Alaboratory specimen for fracture toughness
is usually on the scale of centimeters.For such a specimen,an ‘‘exact’’ 3D simulation using molecular
dynamics or other atomistic methods requires a model that contains about 10
20
atoms,which is beyond
current computational limits.This motivated the development of the ‘‘Quasiparticle dynamics approach’’;
for short,‘‘Particle Dynamics’’.
The basic idea of ‘‘Quasiparticle dynamics approach’’ is to represent an atomic system as a particle
system through lumping ﬁxed number of atoms into a superatom,which we call a ‘‘particle’’,while pre
serving the essential properties of the atomic system via a proposed ‘‘equivalent stiﬀness rule’’.This rule
requires that the particle system has the same crystal structure and stiﬀness coeﬃcients as the original
atomic system but with a larger interparticle spacing that is determined from the scale of interest,see Fig.
10b and c.The original physics is preserved through transforming the interatomic potential (Fig.10a) into
Fig.9.Interfacial metallic debonding/decohesion law.
1
This method is also termed ‘‘Particle Dynamics’’ in other publications of the authors.
1878 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
an interparticle potential by preserving the same elastic constants for both systems.More details of the
method can be found in [31].
We reemphasize that the ‘‘particle’’ in ‘‘Quasiparticle dynamics approach’’ is an atomic aggregate and
the number of atoms in the aggregate is determined by the scale of interest.It can represent an inclusion
particle in alloy matrix such as a TiC particle,or just contains a single atom so that the particle system
degenerates to the original crystal.
The ‘‘Quasiparticle dynamics approach’’ is developed based on the two distinct methodologies:The
embeddedatom method (EAM) [32,33] and meshfree methods [34–36].Regarding the literatures of
meshfree methods and other computational methods associated with multiscale numerical approaches,we
refer to [34,35,37–45].Review of meshfree methods can be found in [46],also recently in [47,48].
Fig.10.Quasiparticle dynamics approach (particle dynamics):(a) conventional Lennard–Jones potential;(b) an atomic system with
the equilibrium interatomic distance a
0
;(c) a particle system with the equilibrium interparticle distance Na
0
;the particles at this scale
are termed as ‘‘quasiparticles’’;(d) the structural particle system where each structural particle is lumped into several quasi particles;
all structural particles are partitioned into natural elements deﬁned by grain structure and (e) coupling of the continuum mechanics
solution inside a grain with interfacial solution.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1879
4.1.Particle system and interparticle potential
For metals,the EAM [32,33] is a powerful method among those employed in the family of molecular
dynamics.In EAM the total energy E
tot
of a crystal,Figs.3a or 4a,is expressed as the summation of a
combination E
i
for each individual atom:
E
tot
¼
X
i
E
i
;ð4:1Þ
where E
i
is deﬁned by
E
i
¼ F
i
ðq
h
i
Þ þ
1
2
X
i;j;j6
¼i
U
atom
ij
ðr
ij
Þ;ð4:2Þ
where q
h
i
is the total electron density at atom i associated with the host (i.e.,the rest of the atoms in the
system) and F
i
is a function of q
h
i
;U
atom
ij
ðr
ij
Þ is a pairpotential that is the function of the distance r
ij
between
atoms i and j.
We propose an addition term to (4.2)
E
i
¼ F
i
ðq
h
i
Þ þ
1
2
X
i;j;j6
¼i
U
atom
ij
ðr
ij
Þ þ
X
i;j;k;j6
¼k;
j6
¼i;k6
¼i
G
ijk
ðh
ijk
Þ;ð4:3Þ
where G
ijk
ðh
ijk
Þ is the energy associated with rotation,h
ijk
is the angle between bonds i j and i k.
As suggested in [49],the function F
i
ðq
h
i
Þ in (4.2) can be written as
q
h
i
¼
X
j;j6
¼i
r
0
ij
r
ij
"#
6
and q
0
i
¼
X
j;j6
¼i
1 ð4:4aÞ
and
F
i
ðq
h
i
Þ ¼ ðE
sep
E
empty
Þ 1
m
0
Log
q
h
i
q
0
i
q
h
i
q
0
i
m
0
;ð4:4bÞ
where the superscript ‘‘0’’ denotes the variables,e.g.r
ij
¼ r
0
ij
,at equilibriumcondition;m
0
is a constant to be
determined;E
sep
and E
empty
are atomic separation energy and unrelaxed empty site formation energy,
respectively;where the former is deﬁned by (3.2),the latter is obtained from the results listed in Table 1.A
general approach to determine E
i
according to atomic separation (3.1) is given in [50].
We propose the threebody energy term in the form as
G
ijk
ðh
ijk
Þ ¼ c
US
½ðcos h
ijk
cos h
jki
cos h
kij
Þ
m
1
c
3
;ð4:5Þ
where h
ijk
is the angle between r
ij
and r
ik
,r
ij
denotes the vector starting at atomi and ends at atomj;m
1
¼ 1
and c
3
¼ 0:1887 for bccFe crystal.
For the atomic systemshown in Fig.10b,in general,the pair potential U
atom
ij
ðr
ij
Þ can be characterized by
the Lennard–Jones potential (Fig.10a):
U
atom
ij
¼ 4e
0
r
0
r
ij
12
"
r
0
r
ij
6
#
ð4:6Þ
which contains two scaling parameters r
0
and e
0
.The former is the ‘‘collision diameter’’ that refers to the
separation for which the energy is zero;and the latter is the ‘‘depth of the well’’ as demonstrated in Fig.10a.
1880 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
Thus,the atomic system in Fig.10b is completely deﬁned when its crystal structure is given with a ﬁxed
potential (4.1)–(4.5).Consequently,when the aggregate particle system in Fig.10c has the same crystal
structure as the system in Fig.10b with a similar interparticle potential like (4.1)–(4.5),then the particle
systemcan be used to reproduce the kinetics and dynamics of the systemin Fig.10b with the accuracy up to
the spacing between the particles.The keyissue here is to ﬁnd the parameters r
0
and e
0
in the interparticle
potential for the aggregated system so as to preserves the same stiﬀness coeﬃcients of the atomic system.
For a cubic system such as bcc and fcc,the crystal stiﬀness is determined by three independent elastic
constants:C
11
,C
12
,and C
44
[32,33].For a given cubic crystal,the parameters r
0
and e
0
,together with the m
0
in (4.4b) can be ﬁxed by these elastic constants,and vice versa.We use the same concept to develop an
‘‘equivalent stiﬀness rule’’ for the ‘‘Quasiparticle dynamics approach’’,i.e.so that the aggregate particle
system has the same stiﬀness coeﬃcients as the underlying crystal.
In this analysis,Roses relation (3.1) is used to ﬁt (4.4) and (4.6) for an atomic systemlike Fig.10b while
m
0
is set to be 0.36 according to results in [51,52].The system in Fig.10b is partitioned into several sub
domains and the atoms in each subdomain are lumped into a single particle,as illustrated in Fig.10c.The
size of each subdomain is determined by the length scale of interest.The ‘‘equivalent stiﬀness rule’’ is
applied to establish the potential for this ‘‘Quasiparticle dynamics approach’’ system.
For simpliﬁcation,here we consider the case of inﬁnitesimal deformation without relative rotation.
There is no diﬃculty to extend this procedure to the ﬁnite deformation case.For an inﬁnitesimal motion of
an atom i in a crystal characterized by (4.2),the change of the energy DE
i
associated with the atom i is
DE
i
¼ F
i
q
h
i
F
i
q
h0
i
þ
1
2
X
j
U
atom
ij
ðr
ij
Þ
h
U
atom
ij
ðr
0
ij
Þ
i
;ð4:7Þ
where j is summed over all neighbors of i if r
ij
is less than a given cutoﬀ radius.The term
F
i
ðq
h0
i
Þ þ
1
2
P
j
½U
atom
ij
ðr
0
ij
Þ denotes a reference state and is a constant.The derivation operations of DE
i
with
respect to the distances to neighbor atoms along a given direction reﬂects the stiﬀness of the crystal in this
direction,which is interpreted as an orientation dependent elastic constant [32].When the system is under
pure volumetric,rhombohedral shear,and tetragonal shear deformation,respectively,one can derive the
corresponding bulk modulus K,rhombohedral shear modulus G
1
and tetragonal shear modulus G
2
.This
provides three conditions to calibrate R
0
,E
0
,and M
0
for the EAMtype energy for the Quasiparticle
dynamics approach system in Fig.10c:
E
QP
i
¼ F
i
ðK
h
i
Þ þ
1
2
X
i;j;j6
¼i
U
QP
ij
ðR
ij
Þ ð4:8Þ
through preserving the same K,G
1
and G
2
as that in the underlying crystal.In (4.8) the superscript ‘‘QP’’
refers to quantities in the Quasiparticle system such as in Fig.10c,and
K
h
i
¼
X
j;j6
¼i
R
0
ij
R
ij
"#
6
:ð4:9Þ
For a bcc or fcc crystal,this transformation can be derived analytically according to crystal distortions [53].
In this study,the proposed ‘‘Quasiparticle dynamics approach’’ is applied for two objectors:bccFe matrix
and TiC–Fe interface.In the former the EAMpotential (4.4)–(4.6) are used where m
0
¼ 0:36;for the latter
only the pair potential (4.6) is applied as m
0
is set to be zero.The TiC matrix is considered to be continuum
elasticity.To illustrate we consider the case that m
0
¼ 0 in bulk iron matrix so the ﬁrst termof (4.8) vanishes
and only the calibrations of r
0
and e
0
are required.
Consider a bcc crystal with lattice constants fa
1
;a
2
;a
3
g;at the equilibrium state,a
i
¼ a
0
,for i ¼ 1;2;3.
Any atom in such a bcc crystal has eight neighbor atoms at a distance of r
1
¼ a
0
ﬃﬃﬃ
3
p
=2,six neighbors at a
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1881
distance of r
2
¼ a
0
,eight neighbor atoms at a distance r
3
¼ a
0
ﬃﬃﬃ
2
p
.In order to illustrate the concept,we cut
oﬀ the ‘‘domain of inﬂuence’’ of the potentials (4.6) to be less than r
3
.
When the crystal is under volumetric deformation
a
1
¼ a
2
¼ a
3
¼ a ð4:10Þ
and the bulk modulus at the position that the atom i occupies is
K
atom
¼
1
9ða
0
Þ
2
½3a
0
ðU
atom
i1
ðr
1
ÞÞ
00
þ3a
0
ðU
atom
i2
ðr
2
ÞÞ
00
4
ﬃﬃﬃ
3
p
ðU
atom
i1
ðr
1
ÞÞ
0
6ðU
atom
i2
ðr
2
ÞÞ
0
;ð4:11Þ
where
ðUðxÞÞ
0
¼
dðUðxÞÞ
dx
and ðU
atom
ij
ðr
j
ÞÞ denotes the potential (4.6) of atom i to the neighbor with the distance r
j
,j ¼ 1;2.For
inﬁnitesimal strain,K
atom
is constant because
ðU
atom
a1
ðr
1
ÞÞ
0
¼ U
atom
a1
a
0
ﬃﬃﬃ
3
p
2
! !
0
;ðU
atom
a2
ðr
2
ÞÞ
0
¼ ðU
atom
a2
ða
0
ÞÞ
0
:
Similarly,when the bcc crystal is under a rhombohedral shear deformation
a
1
¼ a;a
2
¼ a
3
¼ 2a
0
a ð4:12Þ
and the corresponding rhombohedral shear modulus at site i is
G
atom
¼
1
9ða
0
Þ
2
½3a
0
ðU
atom
i1
ðr
1
ÞÞ
00
þ4
ﬃﬃﬃ
3
p
ðU
atom
i1
ðr
1
ÞÞ
0
þ9ðU
atom
i2
ðr
2
ÞÞ
0
:ð4:13Þ
The bcc atomic crystal of Fig.10b is aggregated into a ‘‘bcc quasiparticle crystal’’ with spacing Na
0
in
Fig.10c.This quasiparticle system is characterized by the potential
U
QP
ij
¼ 4E
0
R
0
R
ij
12
"
R
0
R
ij
6
#
;ð4:14Þ
where R
ij
is the distance between a quasiparticles pair i and j.By restricting the domain of inﬂuence of
(4.14) to the ﬁrst two closest neighborparticles and repeating the procedure (4.10)–(4.13),we obtain
K
QP
¼
1
9ðNa
0
Þ
2
½3Na
0
ðU
QP
ij
ðR
1
ÞÞ
00
þ3Na
0
ðU
QP
ij
ðR
2
ÞÞ
00
4
ﬃﬃﬃ
3
p
ðU
QP
ij
ðR
1
ÞÞ
0
6ðU
QP
ij
ðR
2
ÞÞ
0
ð4:15Þ
and
G
QP
¼
1
9ðNa
0
Þ
2
½3Na
0
ðU
QP
ij
ðR
1
ÞÞ
00
þ4
ﬃﬃﬃ
3
p
ðU
QP
ij
ðR
1
ÞÞ
0
þ9ðU
QP
ij
ðR
2
ÞÞ
0
;ð4:16Þ
where
R
1
¼ Na
0
ﬃﬃﬃ
3
p
2
;R
2
¼ Na
0
:
Now introduce the equivalent stiﬀness rule by setting
K
QP
¼ K
atom
;G
QP
¼ G
atom
:ð4:17Þ
These two equations determine the parameters E
0
and R
0
in the particle potential deﬁned by (4.14).
1882 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
At the Fe–TiC interface shown in Fig.3a where Fe is bcc and TiC has the (NaCl)fcc crystal structure,we
assume two classes of quasiparticle potentials:the potentials for the bulk Fe or TiC matrix and interfacial
potential.Eqs.(4.10)–(4.17) describe the procedure to obtain the quasiparticle dynamics potential of bulk
bcciron crystal.The TiC matrix is presumed pure elasticity.
The proposed ‘‘equivalent stiﬀness rule’’ is also applied for determining the quasiparticle interfacial
potential.The interatomic potential at TiC–Fe interface has already been obtained in Section 3,shown in
Figs.4b and 9.The elastic constant associated with the direction perpendicular to the interface,denoted as
C
Fe–TiC
?
,is calculated by the second order derivative of (3.1) [13]
C
FeTiC
?
¼
2c
F
l
atom
d
2
E
N
dk
2
N
TiC–Fe
;ð4:18Þ
where l
atom
is the interfacial interplanar spacing of the atomic system at equilibrium state,see
Table 1.Using (4.6) to describe (3.1),r
0
an e
0
of (4.6) are determined according to l
atom
and total decohesion
energy.
Assuming that l
QP
,the interfacial interplanar spacing for the quasiparticle dynamics approach systemat
equilibrium state,is given by
l
QP
¼ Nl
atom
;ð4:19Þ
where N is deﬁned in Fig.10c;we have
C
FeTiC
?
¼ l
QP
d
2
U
QP
dR
2
;ð4:20Þ
where U
QP
is the quasiparticle interfacial potential.
By comparing (4.20) with (4.18),together with (4.19),we have two relations to calculate the parameters
in U
QP
deﬁned by (4.14).
4.2.Coupling of quasiparticle dynamics approach and continuum mechanics
Here,we propose a procedure that couples the ‘‘quasiparticle dynamics approach’’ with the continuum
mechanics simulation.
To aﬀect the coupling behavior between the discrete quasiparticle representation and a continuum,a
lumping procedure similar to that employed in quasicontinuum method [54,55] is used.Using meshfree
method,each grain or inclusion particle is discretized into several nodes that are termed ‘‘structural par
ticles’’.Each structural particle is lumped by several quasi particles,as illustrated in Fig.10d.The quantities
associated with a structural particle I is denoted by the capital subscript I and the quantities associated with
a quasiparticle i is denoted by the plain subscript i.
We assume that the velocity ﬁeld
_
u for the problems in Fig.10d–e can be written as an multilevel
decomposition [38,40,44,56]
_
u ¼
_
u
C
þ
_
u
SP
_
w;ð4:21Þ
where
_
u
C
is the continuum velocity ﬁeld,
_
u
SP
the velocity ﬁeld described by discretized nodes (structural
particles) and
_
w the overlapping velocity ﬁeld bridging continuumand particle scale.For application of this
approach,see [40,44,56–58],also in [59],where a introduction is given to associated with other approaches.
The continuum mechanical solution
_
u
C
is determined through the total Lagrange weak form [60]
Z
X
I
q
C
0
d
_
u
C
þsðu
C
Þ:rd
_
u
C
dX
I
Z
C
I
t
t d
_
u
C
dC
I
t
¼ 0;ð4:22Þ
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1883
where q
0
is the density at reference conﬁguration and s is the ﬁrst Piola–Kirchhoﬀ stress tensor,X
I
is a
reference domain that coincides to the grain I in Fig.10d and e,C
I
t
is the boundary of X
I
where the traction
t is applied.In a discretized ‘‘structural particle’’ system,the last term in (4.16) is expressed in the form as
Z
C
I
t
t d
_
u
C
dC
I
t
¼
X
N
J
J¼1
w
J
t
J
d
_
u
C
J
;ð4:23Þ
where the subscript ‘‘J’’ denotes the quantities at node J and w
J
is the weight at this node;there are in total
N
J
nodes (structural particles) in X
I
on which the force
t
J
is imposed.The moving particle ﬁnite element
method is applied to solve (4.22) and (4.23) in each X
I
and the interaction between X
I
1
and X
I
2
is governed
by the interfacial potential deﬁned in (4.24) as below.
The solution of (4.22) requires knowledge of a constitutive relation,which can be obtained in two ways:
to deﬁne a structural particle pair potential using the same procedure for quasi particles and to engage a
continuumanalytical model [61] based on the Cauchy–Born law.The second way is applied in this analysis.
The details will be given in the following sections.
The u
SP
is solved using the potential deﬁned below.Let X
I
1
;X
I
2
;X
I
3
...be the domain of the grains
I
1
;I
2
;I
3
;...(the subdomain of the secondary partitioning in Fig.10d);the pair potential between a
structural particle J
1
in X
I
1
and another structural particle J
2
in X
I
2
is deﬁned as
U
SP
J
1
J
2
¼
P
N
J1
i¼1
P
N
J2
j¼1
U
QP
ij
ðR
ij
Þ for X
I
1
6
¼ X
I
2
;
0 for X
I
1
X
I
2
;
ð4:24Þ
where U
SP
J
1
J
2
is the pair potential in the structural particle system and U
QP
ij
ðR
ij
Þ is the pair potential between
the quasiparticle i that is lumped to the structural particle J
1
and the quasiparticle j is lumped to the
structural particle J
2
;N
J1
and N
J2
denote the number of quasiparticles lumped to J
1
and J
2
,respectively.At
Fe–TiC interface,the U
QP
ij
is determined according to (4.18)–(4.20).
The potential U
SP
J
1
J
2
in (4.24) establishes the bonds between X
I
1
and X
I
2
.Hence,the solution of u
SP
provides the boundary condition of u
C
,as illustrated in Fig.10e.
To trade oﬀ the overlapping between u
SP
and u
C
,the term
_
w in (4.21) is deﬁned as
_
w ¼
_
u
C
at structural node J
1
:U
SP
J
1
J
i
6¼ 0;
0 at structural node J
1
:U
SP
J
1
J
i
0:
(
ð4:25Þ
Thus,the boundary value problem deﬁned in Fig.10e is solved through the continuum mechanics weak
form (4.22) with the boundary conditions deﬁned by (4.23) and (4.24).
5.Hierarchical unit cells and constitutive model
In this section we discuss the response of the submicro unit cell and microcell models with secondary
and primary inclusions by employing the ﬁrst principlebased potential obtained in the previous sections.
The procedure summarized in Figs.1 and 2 is engaged in this analysis.The resulting macroscale consti
tutive law will then be applied in a macroscale simulation of ductile fracture.The experimental results of
modiﬁed 4340 steel [62,63] are used as an example in the simulation.For the constitutive modeling of
heterogeneous system,we refer [64–80].
5.1.A thermodynamic framework for multiphysics computational mechanics
First we establish a thermodynamic framework for computational mechanics analysis based on the
theory of Hughes [81],which provides the necessary conditions for
1884 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
• setting up a constitutive model without violation of the energy conservation law
• conducting a stabilized numerical simulation.
In the following analysis,we use r to represent the Cauchy stress tensor and
_
the symmetric part of the
velocity gradient.Both the Cauchy stresses and velocity gradient can be at either submicro,micro,or
macroscale.All analysis will be performed in a corotation conﬁguration so the change of stress due to
system rotation is removed.The notations and formulations of continuum plasticity introduced in [60] are
applied in this analysis.The detailed formulation of the corotation operation under large deformation is
introduced in Appendix B.
We assume the additive decomposition of strain rate
_
_
¼
_
e
þ
_
p
;ð5:1Þ
where the superscript ‘‘e’’ denotes the elastic part and ‘‘p’’ denotes the plastic part.More explanation about
(5.1) is introduced in Appendix C.
In conventional continuum plasticity
_
r ¼ D
e
:
_
e
;
_
p
¼
_
e
oU
or
;ð5:2Þ
where D
e
is elastic stiﬀness matrix,
_
e is ‘‘ﬂow factor’’,U is the plastic potential to be found
U ¼ Uðr;k
1
;k
2
;...;k
m
Þ;ð5:3Þ
where k
k
are internal variables,such as equivalent plastic strain,damage,etc.
Following the conventional elastic–plastic analysis,e.g.the procedure introduced in [60],(5.7) leads to
the incremental formulation of constitutive law when U is known:
Dr ¼ D
ep
:D
_
;
where
D
ep
¼ D
e
ðD
e
:U
r
ÞðU
r
:D
e
Þ
P
k
h
k
U
k
k
þU
r
:D
e
:U
r
ð5:4Þ
and
U
k
k
¼
oU
ok
k
;U
r
¼
oU
or
;
_
k
k
¼
_
eh
k
¼
_
e
oW
k
oF
k
;
where F
k
,k
k
are conjugate pairs of the internal variables in (5.3) and the corresponding general thermo
dynamic force,respectively.For example,F
k
,k
k
can be the pair of stress r and strain ,the interfacial
traction
t and separation ½u,a scale damage f and its driving force h,temperature gradient and heat ﬂux,
etc.W
k
is the corresponding energy dissipation of the pair ðF
k
;k
k
Þ
W
k
¼
Z
k
k
0
F
k
dk
k
:ð5:5Þ
We want to ﬁnd the general rule to establish a potential U in (5.2) for a system with multiphysics.
Hughes [81] has proven that the stability of a computation mechanics solution is determined by the sat
isfaction of the local form of the Clausius–Duhem inequality
X
k
½F
k
_
k
k
_
W
k
ð
_
k
k
;TÞ
_
uð
_
e
;TÞ þs
_
T P0;ð5:6Þ
where T,s,u denote in turn the temperature,entropy,and free energy.The Clausius–Duhem inequality is
actually an alternative representation of the second thermodynamic principle [82],which has been widely
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1885
applied in the constitutive models,e.g.in [82–84].However,only [81] reveals that (5.6) is equally important
for both constitutive modeling and numerical simulation,which is crucial for computational material de
sign.
In this analysis we assume no heat supply and conduction.Considering the simplest case in Fig.10e:only
the conjugate pairs of stress–strain ðr;Þ,interfacial traction and separation ð
t;½uÞ,scale damage and its
driving force ðh;f Þ,are taken into account;then (5.6) becomes
r:
_
þt ½
_
u þh
_
f
_
uð
_
e
;TÞ
_
W
t
_
W
f
þs
_
T P0;ð5:7Þ
where W
t
and W
f
are the energy dissipations of ð
t;½uÞ and ðh;f Þ,respectively;and
_
u ¼
ou
o
e
:
_
e
þ
ou
oT
_
T;
_
W
t
¼
oW
t
o½u
:½
_
u þ
oW
t
oT
_
T;
_
W
f
¼
oW
f
of
_
f þ
oW
f
oT
_
T:ð5:8Þ
On the other hand
r ¼
ou
o
e
;s ¼
ou
oT
þ
oW
f
oT
þ
oW
t
oT
:ð5:9Þ
Substituting (5.8) and (5.9) into (5.7),it can be satisﬁed if
t ¼
oW
t
o½u
;h
f
¼
oW
f
of
ð5:10Þ
and
r:ð
_
_
e
Þ P0:ð5:11Þ
The ﬁrst relation in (5.10) requires W
t
to be Needlemans potential,e.g.deﬁned by (4.24).The second
relation of (5.10) deﬁnes a potential of damage.By comparison (5.11) with (5.2),we obtain
_
r:
oU
or
P0:ð5:12Þ
This equation lays down a ‘‘convex condition’’ for any proposed plastic potential U,which also deﬁnes the
local form of stability condition for the multiphysics computational mechanics approach.At a material
point,(5.12) is an alternate expression of Druckers postulate for isotropic plasticity.
5.2.Twolevel cell modeling
The cell models for determining the constitutive response are based on periodic distributions of inclusion
particles.Hence,according to the arrangements of the inclusions,three representative cells are illustrated in
Fig.11a.Using periodic and symmetric properties,the threedimensional cubical primitive distribution can
be simpliﬁed to the twodimensional rectangular cell with single inclusion;whereas the 3D body central
cubic or hexagonal distribution can be simpliﬁed to the 2D rectangular cell with double inclusions,as
shown in Fig.11b.By varying the shape,size and distributions of the primary/secondary inclusion particles
and the decohesion energies,the methodology of computational cell modeling introduced,e.g.in
[67,69,70,74,85],is applied in this paper.
The Bishop–Hill relations [86]
R
ij
¼
1
V
cell
Z
V
cell
r
cell
ij
dV;
_
E
ij
¼
1
V
cell
Z
V
cell
_
e
cell
ij
dV ð5:13Þ
are employed in the analysis which establishes the relationship between the homogenized average stress/
strain (R
ij
;E
ij
) response and cell stress/strain (r
cell
ij
;e
cell
ij
).The amplitudes and distributions of r
cell
ij
;e
cell
ij
are
1886 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
determined by parameters such as the material properties of the cell matrix and inclusion,the interfacial
cohesion,the size and geometries of inclusions,and the load imposed on the cell.Both two dimensional and
three dimensional cells are analyzed.
5.2.1.Submicrocell model
The submicrocell simulation aims to:
(1) investigating the eﬀects of the secondary inclusion particles (TiC,about 2–300 nm in size) and debond
ing behavior on the microstress–strain response;
(2) establishing the corresponding constitutive model that is applied as the matrix material in a microscale
cell model.
The quasiparticle dynamics approach is applied in the submicroscale cell model.At the structural
particles level (Fig.10d and e),the entire iron matrix is treated as a grain and the inclusions are to be other
grains.The interfacial decohesion curves shown in Fig.9 are applied for establishing the particle potential
(4.24).The secondary particle,TiC,is treated as isotropic and linear elastic with the Youngs modulus of
600 GPa and a Poisson ratio 0.3.
A crucial part of this simulation is to establish the constitutive law of the iron matrix.According to the
ﬁrst principle calculation,the (1 11) adhesion energy of pure iron is about 5.5 J/M
2
which leads to a peak
decohesion stress around 45 GPa,see Table 1 and Fig.12a.When point defects,e.g.empty sites,exist,the
adhesion energy drops drastically,see Table 1.Using the homogenization procedure,e.g.[61,87],the
Fig.11.The cell model:(a) three classes of periodic distributions of inclusions and (b) boundary conditions imposed in cell modeling.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1887
interatomic force separation relation in Fig.12a can be transformed to an nonlinear elastic constitutive law
shown in Fig.12c.
On the other hand,the analysis of Section 3 indicates that a bcciron is ‘‘intrinsically ductile’’ according
to (3.3) and the model introduced in Fig.5.The corresponding shear traction vs.gliding separation is
shown in Fig.12b.Applying the model illustrated in Fig.7 to the separation of iron matrix,one can ﬁnd
that the gliding induced dislocation has two obvious eﬀects on the corresponding homogenized stress–strain
Fig.12.The constitutive law of iron matrix,from interatomic forceseparation relation to conventional plasticity:(a) interatomic
normal traction vs.separation;(b) interatomic shear force vs.gliding;(c) a nonlinear elasticity,homogenized based on (a);(d) a stress–
strain response homogenized combining normal separation and gliding,and J
2
plasticity and (e) experimental measurement of the
modiﬁed 4340 steel [62,63].
1888 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
response:(1) reducing peak stress;(2) increasing the strain at ﬁnal failure,as show in Fig.12d.Fig.12a–d
actually explain how plasticity occurs in real steel.Theoretically speaking,the amplitude of the ‘‘yield
plateau’’ and the value of the ﬁnal failure strain in Fig.12d can be computed accurately using ﬁrstprinciple
computation.However,in practice it is diﬃcult to know the exact numbers and positions of point defects
because these parameters actually determine the ﬁnal result.
In this research the iron matrix of submicrocell is assumed to be a continuum medium governed by
the stress–strain response with a ﬂat ‘‘plateau’’ in Fig.12d.The homogenization of the atomic normal
separation,plotted in Fig.12c,is split into two parts to describe loading stage I and softening stage III
in Fig.12d,respectively;whereas the J
2
plasticity is applied to describe the stage II,i.e.the ‘‘plateau’’.
The experiment result of the modiﬁed 4330 steel [62,63] is applied to calibrate the height of the
‘‘plateau’’ and the onset of softening,denoted as the yield strength r
Y0
and the shear failure strain e
f
,
respectively.
Fig.12e shows the experimental stress–strain curve of the modiﬁed 4340 steel,which is studied in col
laboration with the Caterpillar Technical Center employing both uniaxial tension and pure shear tests
[62,63].Under the pure shear condition,no signiﬁcant debonding between the primary inclusions and the
alloy matrix has been observed and the material fails entirely by microvoiding at the secondary particles;
therefore the measured initial yield stress is taken as a lower bound whereas the maximum stress is as an
upper bound of the yield strength of the iron matrix since the measured result contains the strengthening
provided by the secondary (TiC) particles after yielding in the steel.
In the computation the initial slope at stage I,which deﬁnes Youngs modulus,is 200 GPa with a Poisson
ratio of 0.3.The r
Y0
,measured at initial yield in the experimental stress–strain curve,is 1.03 GPa and the
failure shear strain is 0.2 according to shear test.
In the submicrocell modeling,biaxial tension (2D) and triaxial tension (3D) are imposed on the unit cell.
Various ratios of the ﬁrst and the third principle stresses are chosen to reproduce uniaxial tension,pure
shear,and the stress state inbetween.The average stresses and strain are measured according to (5.13).
Plotted in Fig.13 are a set of snapshots of the submicro equivalent plastic strain contours during
debonding and the corresponding microshear stress–strain response.The cell is under shear dominant
boundary conditions.However,a localized normal separation may also occur.These results demonstrate
that the localization incipience is characterized by onset of the shear bands connecting two inclusions,it
triggers a subsequent fast debonding along the interface and results a sudden drop of the microscale stress.
This phenomenon is quite close to the model and the associated hypotheses in Fig.7,which illustrates that
normal separation is a combination of the normal components of gliding induced dislocation and the
separation between interfacial atompairs.For an intrinsically ductile material like bccFe,gliding induced
dislocations motion dominates.Fig.14 shows an experimental observation which demonstrates that a shear
band induces the coalescence of microvoids.
It is well known that parameters such as volume fraction,orientation and distribution of the secondary
particles,as well as stress state and decohesion energy,determine the submicrocells deformation and
failure behavior.According to the computational results plotted in Fig.13,we conclude that among these
parameters,the decohesion energy is particularly important.Plotted in Fig.15 is a set of computations
where the decohesion energy varies from zero to the upper bound value corresponding to the Fe–C site
conﬁguration (see Fig.3b).In these computations,spacing and volume fraction of the secondary particles
are ﬁxed.If we use the microscale strain E
micro
12
at debonding as a threshold value for the microstress–strain
relation,then from Fig.15 we ﬁnd that this debonding strain increases substantially when the decohesion
energy increases.When the decohesion energy reaches its upper bound (3.8 J/m
2
),no debonding takes place
at all.
Fig.16 shows a 3D simulation performed by ﬁnite element method.The cell is under uniaxial tension
with the interfacial decohesion energy 0.6 J/m
2
.This simulation is used to test the model and the parameters
setup.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1889
Based on a large amount of numerical simulation and the methodology of cell modeling introduced in
[88],a general framework of multiscale constitutive model has been developed,which couples interfacial
debonding,void nucleation and growth,localization with strain gradient eﬀects and phase transformation.
For an isotropic material,the corresponding plastic potential is expressed as
Fig.13.Snapshots of the localization induced debonding process.
Fig.14.Observation:localization induced decohesion [J.F.Mescall (US Army Mat.Lab)].
1890 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
U
plasticity
ðf
0
;f;r
ij
Þ ¼
r
r
intr
!
2
þA
0
r
m
r
intr
þA
1
ðf þg
1
Þ exp
r
m
r
intr
þA
2
ðf þg
2
Þ exp
r
m
r
intr
ðq
0
þq
1
ðf Þ
2
Þ ¼ 0;ð5:14Þ
where r
ij
,
r,r
m
f
0
and f denote in turn the stress tensor,equivalent stress,mean stress,inclusion and void
volume fraction at a given scale;r
intr
denotes the ‘‘material intrinsic strength’’ that contains the eﬀects of
internal variables associated with strain softening in postbifurcation stage;the constants A
i
and q
i
are
calibrated through the cell models.
When the constants A
i
and q
1
in (5.14) vanish,this potential degenerates to the conventional J
2
plasticity
except the yield strength is replaced by ‘‘
ﬃﬃﬃﬃﬃ
q
0
p
r
intr
’’.(5.14) becomes a ‘‘Drucker–Pragerlike’’ plastic potential
when A
0
is nonzero whereas convert to a ‘‘Gursonlike’’ model when A
0
¼ 0 but A
1
¼ A
2
and g
1
¼ g
2
¼ 0.
For modiﬁed 4340 steel,the microscale plastic potential is derived
U
micro
ðf
II
0
;f
II
;R
micro
ij
Þ ¼
R
micro
r
flow
!
2
þðf
ðf
II
ÞÞ
g
g
0
expðv
1
Þ
3r
Y0
r
flow
ð1 þðf
ðf
II
ÞÞ
g
qÞ ¼ 0;ð5:15Þ
Fig.15.The eﬀect of decohesion energy on the global stress–strain curves.
Fig.16.Threedimensional cell modeling.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1891
where
R
micro
and R
micro
m
are the equivalent and mean stress of R
micro
ij
,respectively;f
II
0
is the volume fraction of
the secondary particles,f
II
is the volume fraction of the voids nucleated from f
II
0
,f
ðf
II
Þ is the damage
evolution function deﬁned by Tvergaard [89]
f
ðf
II
Þ ¼
0 f
II
< f
II
0
f
II
f
II
0
6f
II
< f
II
c
f
II
c
þK
II
ðf
II
f
II
c
Þ f
II
Pf
II
c
8
>
<
>
:
ð5:16Þ
and the v
1
in (5.15) are the functions deﬁned as
v
1
¼ a
1
f
R
micro
m
R
c
max
r
Y0
þa
2
f
R
micro
R
US
max
r
Y0
!
;ð5:17Þ
where R
micro
m
is the mean stress of R
micro
ij
;a
1
and a
2
are constants,a
1
¼ 1:06,a
2
¼ 0:3.R
c
max
is the strength
against the normal separation of the interface between alloy matrix and secondary particles,i.e.,the peak
stress in traction–separation law in Fig.10.R
US
max
is the shear strength against gliding induced dislocation.
The function f in (5.17) is deﬁned as follows:
fðxÞ ¼
x if x P0;
0 otherwise:
ð5:18Þ
The constants in (5.15)–(5.18) are listed in Table 2.
5.2.2.Microcell model
The constitutive model (5.15) is embedded into the matrix of the cell that contains a primary particle
with a size of around 1–2 lm,as plotted in Fig.17a.This representative unit cell is used to obtain the
macroscale stress–strain relation (R
ij
;E
ij
).In high strength steel,e.g.the modiﬁed 4340 [62,63],the primary
particles are typically titanium nitrides (TiN) of cubical shape,represented in the model as square,see Fig.
17a.
Experimental research reveals that the debonding–decohesion between large nitrides and matrix usually
takes place under relative low load level.This is because the accumulation of misﬁt strain and the segregate
impurity elements (mainly the Sulfur) precipitated along the grain boundary can reduce the interfacial
strength signiﬁcantly.The tractionseparation in Fig.9,calibrated according to the peak value given in [63],
is applied in simulation.A typical debondinglocalization phenomenon for this class of cell and the cor
respond slipﬁeld are illustrated in Fig.17c.The TiN is assumed to be elastic with a Youngs modulus of
350 GPa [20] and a Poisson ratio of 0.3.
Plotted in Fig.18 are set of computed macroscale stress–strain curves with varying primary inclusion
volume fraction,where the macroscale stress–strain response demonstrates three stages of the cell behavior:
(I) elastic deformation and yielding;(II) debonding/decohesion between large nitride inclusions and the
alloy matrix;(III) postbifurcation/softening.In contrast to Fig.15,two stress drops appear in stage II.
These are caused by debonding at two perpendicular surfaces of the square nitrides.By varying the shape,
size and distribution of the primary/secondary particles and the decohesion energies,the shape of the
stress–strain curve and positions of the turningpoints between diﬀerent stages vary.These provide the
Table 2
Parameters in (5.15)
g
0
g q a
1
a
2
f
II
c
K
II
1.5 2 )0.33333 1.06 0.2 0.05 3
1892 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
possibility of choosing an optimum combination of particle size,geometry and distribution for micro
structural design.
The stress and strain at the onset of stage III,as well as the slope of the subsequent softening,are key
parameters linked to the failure behavior of the material.A challenge is how to implement the phenomena
reﬂected in Fig.17 into an applicable constitutive law.We discuss this issue in the following section.
5.2.3.Coupling and macroscale constitutive law
To obtain desirable fracture toughness,the stress–strain response after the onset of softening plays a
signiﬁcant role in crack growth simulation,which actually reﬂects the ﬁnal stage of the coalescence of voids.
In the framework proposed in this paper,a concurrent model is introduced and described as follows.
Fig.17.Microscale cell modeling:(a) TiN [1];(b) microscale cell and (c) localization induced decohesion.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1893
Material resistance against void coalescence is determined by the strength of the ligaments between these
voids [88,90].The deformation tolerance and the failure of the matrix ligament are determined by two basic
deformation modes:localization induced necking under normal stress and shear localization caused by the
shear stress component.Consequently,we postulate that the matrix can be divided into two parallel groups
of microscopic elements.The ﬁrst group can be considered as a virtual bond network built in the alloy
matrix;the second group is assumed to be a superposition of imaginary microslices that correspond to the
slip systems along diﬀerent orientations (see Fig.19a–b).In each bond or slice,the strain gradient theory
[91,92]based 1D localization solutions for tension or pure shear [56] are applied.In this class of solution
the material intrinsic length scale l [91,92] is included and the eﬀects of geometrically necessary dislocations
are taken into account.For isotropic materials,a multidimensional stress–strain behavior can be char
acterized through uniaxial and pure shear strain gradient theorybased solutions,which is represented by
the material intrinsic strength r
intr
presented in (5.14).It provides the matrix material properties after the
onset of strain softening in the microscale cell model (see Fig.19c),in conjunction with primary particles
and the subsequent damage evolution.
Based on the concurrent model and numerical results,by rewriting (5.14) at this scale we obtain a
macroscopic plastic potential
U
macro
¼
R
r
intr
2
þA
0
R
m
r
intr
þA
1
ðf
I
þg
1
Þ exp
R
m
r
intr
þA
2
ðf
I
þg
2
Þ exp
R
m
r
intr
ðq
0
þq
1
ðf
I
Þ
2
Þ ¼ 0 ð5:19Þ
and the associated ﬂow law
_
E
p
¼
_
k
oU
macro
oR
;
where
_
k is the ‘‘ﬂow factor’’,
R and R
m
denote the Cauchy equivalent stress and Cauchy mean stress,
respectively;f
I
represents the void volume fraction which is considered as ‘‘damage’’;A
0
,A
1
,A
2
,g
1
,g
2
,q
0
and q
1
are dimensionless material constants listed in Table 3.The evolution laws of damage nucleation and
growth introduced in [93] and the material parameters of the modiﬁed 4340 steel presented in [63] are
applied in this work.
Fig.18.Macroscale stress–strain response with varying volume fracture of nitrides.
1894 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
The plastic potential (5.19) is a macroscale,J
2
like plasticity with damage.The concurrent model
associated with the mechanisms in Figs.18 and 19 is described by ‘‘r
intr
’’ in (5.19),which is termed
‘‘material intrinsic strength’’.It is deﬁned as the combination of a material strain hardening/softening law
and the strain gradientbased traction–separation law:
r
intr
¼
r
Y0
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
r
hom
ð
E
p
Þ
r
Y0
h i
2
þlg
r
strain hardening=softening
E
p
6½
E
bifurc
;
Tð
e
Y;l;gÞ decohesion softening
E
p
> ½
E
bifurc
;
8
<
:
ð5:20Þ
where
E
p
is the plastic part of the equivalent strain and ½
E
bifurc
denotes
E
p
at the bifurcation point of the
r
intr
ð
E
p
Þ relation.Originally l is deﬁned as the material intrinsic length scale deﬁned as the product of
Burgers vector b and the initial yield strength r
Y0
;g is the equivalent strain gradient [92]:
Fig.19.Two microscopic elements:virtual bond and shear slice.
Table 3
Parameters in (5.19)
A
0
A
1
A
2
g
1
g
2
q
1
q
0
0.0666 0.85 1.7 0.01 0.01 2.65 1.0255
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1895
l ¼ 3
E
r
Y0
2
b;g ¼
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
1
2
u
k;ij
u
k;ij
r
;ð5:21Þ
where E is Youngs modulus;and the strainlike parameter
e
Y is deﬁned by
e
Y ¼ ð
E
p
½
E
bifur
Þ
l
l
0
;ð5:22Þ
where l
0
is a material constant,of the same order as the spacing between primary particles.½
E
bifurc
marks
the transition between the two stages of deformation:the uniformdeformation with damage nucleation and
growth and the failure of the ligaments between these defects.½
E
bifurc
can be calibrated to the maximum
stress on the r
intr
ð
E
p
Þ curve fromthe uniaxial tension test.During the second stage,the eﬀect of the material
intrinsic length scale,strain gradient,and strain rate are incorporated in r
intr
as
T ¼ r
Y0
e
T ð
E
p
;l;l
0
Þ
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
r
hom
ð
E
p
Þ
r
Y0
2
þlg
s
:ð5:23Þ
The second termin (5.23) is the traction–separation law derived fromthe strain gradientbased localization
solution at the microscale;the third and fourth terms reﬂect,in turn,the strain rate eﬀect and the material
hardening due to the strain gradient at macroscale.As the microscale localization,representing ligament
failure,is described by
e
T in (5.23),the stress–strain response without bifurcation,denoted by r
hom
ð
E
p
Þ,
appears under the square root of the fourth term.
Based on the analytical solution described in [88],a ﬁtted expression of
e
T can be expressed as
e
T ¼
0:5398Y
2
þ1:5867Y 0:0466
1 k
tr
;ð5:24Þ
where
Y ¼ exp 10
6
ð
e
Y Þ
11=5
n o
;k
tr
¼
r
I
3r
m
2r
I
and k
tr
< 1:
According (5.1) and (5.2),the plastic part of macroscale strain is determined by the potential (5.19) and
elastic part is determined by Hooks law.As the iron matrix and inclusion particles have diﬀerent Youngs
modulus,a formula to estimate macroscale Youngs modulus is suggested in the form as
E
macro
¼ v
Fe
E
Fe
þv
TiC
E
TiC
þv
TiN
E
TiN
;ð5:25Þ
where ‘‘v
X
’’ denotes the volume fraction of X and E
X
is the Youngs modulus of X.For all components a
Poissons ratio of 0.3 is applied.
6.Laboratory specimen scale:Simulation,results,and discussion
6.1.Fracture toughness simulation
In this section we describe ductile fracture simulation carried out on a center cracked panel according to
the ASTM Standard E399E1737,which has been applied in the simulations in [85,95],using the hierar
chical constitutive model developed in the previous sections and the meshfree code [34,35,96].As discussed
in [72,95],the loading speed and materials strain rate sensitivity may have a strong eﬀect on damage
evolution,thus,fracture toughness.However,in this paper only the results under quasistatic loading are
presented.
1896 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
Fig.20 presents two snapshots of 3Dcrack propagation using the macroscale plastic potential described
in (5.19).Fig.21a shows the contours of equivalent plastic strain around a blunted crack tip at smallscale
yielding,where the RiceJohnson type crack tip strain ﬁeld is present.Fig.21b shows the contours after
considerable crack growth with large deformation.In this computation the primary particles (TiN) are
explicitly embedded into the matrix that includes the secondary particles so that the microscale plastic
potential (5.14),in conjunction with the (4.24) in quasiparticle dynamics approach,is applied.Plotted in
Fig.21c is the corresponding load–CTOD curve,where a black square indicates the CTOD at crack ini
tiation which deﬁnes the fracture toughness of the material.Figs.20 and 21 demonstrates that the com
putational approach is capable of capturing this class of phenomenon.On the other hand,it also reveals
that the computational results depend upon many factors such as the geometry and distribution of
inclusions,which are not readily captured by the periodic cell models in Fig.11.
6.2.Ductile fracture simulator and toughnessstrengthadhesion diagram
The hierarchical constitutive and computational methodology introduced in this paper results in a
‘‘ductile fracture simulator’’,illustrated in Fig.22.Starting from the leftlower corner,the quantum
mechanics analysis explores the fundamental atomistic–electronic structures of the alloy matrix and the
matrix/inclusion interface.This provides the corresponding energy–adhesion relations that are applied in
the submicro and microcell modeling to obtain the corresponding constitutive relations (5.14),(5.15),
(5.19) for the matrix material in each scale.For the modiﬁed 4340 steel,the computational results have been
calibrated by experiments.The constitutive law (5.19) of a inclusion induced voiding/microvoiding steel is
implemented into compute codes for calculating crack parameters such as the crack tip opening dis
placement (COD,see Fig.21a) and the Jintegral using the method introduced in [97,98].The COD (or
Jintegral) at crack growth initiation represents the fracture toughness of the material according to the
ASTM standard.The simulated results are summarized by the toughness–strength–adhesion (TSA) dia
gram that is at the rightupper corner of Fig.22,which provides insight into the correlations between the
steel strength,interfacial decohesion,and fracture toughness.
The TSAdiagramat the rightupper corner of Fig.22 is detailed in Fig.23.In Fig.23a the ﬁrst principle
based traction–separation relations are plotted at various adhesion energy levels.Obviously higher
Fig.20.The strain gradient theorybased strain softening solution for the microscopic elements in Fig.19,where l denotes the
microscale length [92] that scales the dissipation during postbifurcation deformation [56] and l
0
denotes the average spacing between
primary particles.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1897
adhesion energy results in higher peak decohesion stress.Fig.23b is the TSA diagramcorresponding to the
TSA curves presented in Fig.23a.
In the TSA diagram(Fig.23b) the dashed lines represent the computed load–COD curves for the center
cracked panel under tension.Simulations with values of matrix yield strengths of 500,700,900 and 1030
MPa are performed using the proposed hierarchical multiphysics constitutive models (5.14),(5.15) and
(5.19).Along each dashed line the circle,delta,solid circle,and triangle denote in turn the CODi (the COD
at crack growth initiation),corresponding to the diﬀerent levels of decohesion energy of the interface be
tween the iron matrix and the inclusion particles,illustrated in Fig.23a.The solid lines indicate the vari
ation of fracture toughness when the decohesion energy is ﬁxed but the strength of the iron matrix is varied.
For example,at the decohesion energy of 0.6 J/m
2
,the most right circle denotes the CODat crack initiation
for the matrix with the yield strength of 1.1 GPa.Similarly,the most left circle on the line with 0.6 J/m
2
denotes the COD at crack initiation for the steel with the matrix yield strength 0.5 GPa.
In the simulations presented in the TSAdiagramthe diameters of the primary TiNparticles ranged from
1 to 2 lm with a volume fraction from 0.02% to 0.2%;the diameters of the secondary particles are from 20
to 200 nm with a volume fraction from 0.02% to 0.4%.The computation shows that crack propagation is
mainly governed by the decohesion–debonding process of the primary TiN particles (inclusions) whereas a
uniformly distributed small inclusion particles have a relatively stronger eﬀect on strengthening,rather than
on fracture.More detailed investigations,especially for the system with nonuniformly distributed inclu
sions,are required for clarifying the dual eﬀects of secondary particles on strengthening and toughness.
Fig.21.A simulation of crack growth:contours of equivalent stress and load–CTOD curve.
1898 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
Fig.23b reveals that increasing adhesion energy is a way to improve fracture toughness while main
taining strength.However,the TSA diagram also indicates that the toughening eﬀect of adhesion energy is
relatively reduced at high strength.Apparently,ﬁxing interfacial strength but varying alloy matrix strength
or verse versa may have a similar eﬀect on fracture toughness.The trend obtained from the TSA diagram
coincides with several experimental reports,e.g.[24,99–102].
The TSA diagram in Fig.23b,in conjunction with the analyses presented in the previous sections,
provides several guidelines for steel design:
(1) Both interfacial adhesion energy and strength ratio are crucial for obtaining high toughness with high
strength.A quantitative description of these relationships is given in Fig.23.
(2) Large inclusions (>1 lm) can not maintain high interfacial strength and is the major cause of lower
toughness.
(3) For smaller dispersed particles,dispersion spatial uniformly may be particular important for enhanced
toughness.
(4) The densities of point defects in an alloy matrix,such as vacancies,dislocations,have strong ef
fects on the strength and fracture mode of the alloy.The ratio between the normal separation
energy and the energy barrier against dislocation motion determines the macroscale strength of
alloys.
Fig.22.Ductile fracture simulator.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1899
7.Conclusions
• At atomistic scale the failure of metal can be caused by two diﬀerent mechanisms:normal separation
between atomic pairs and gliding induced dislocation.Rices criterion of ductilebrittle fracture transi
tion has been applied to determine which of them will occur.
• The density functional theorybased quantum mechanical computation indicates that in bcciron crystal
the gliding induced separation is dominant,which explains why plastic ﬂow takes place.
• A ‘‘quasiparticle dynamics approach’’ approach has been developed and is applied at the scale bridging
quantum physics and continuum mechanics.
• A computational thermodynamic framework of metal plasticity,which unions diﬀerent physics concur
rently,has been developed based on Clausius–Duhem inequality and Hughes stability theory.
• Using a twolevel cell modeling,a hierarchical constitutive model has been developed for the ultrahigh
strength steels that contain the primary inclusion particles about microns in size and the secondary inclu
sion particles about 10 nm in size.
• The simulation of ASTMstandard fracture toughness specimen,at ﬁrst time,leads to a multiscale com
putationbased TSA diagram,which provides a guideline to assist future alloy design.
• The multiscale computation indicates that the densities of point defects in alloy matrix have strong ef
fects on the strength and fracture mode of the alloy.The ratio between the normal separation energy and
the energy barrier against dislocation motion determines the macroscale strength of alloys.
Acknowledgements
The steel design project is funded by ONR (Grant Number:N000140110953).Su Hao is funded by
ONR (1/20037/2003) and by NSF (3/200212/2002).The support of ONR and NSF are greatly appre
ciated.Su Hao thanks Dr.Singh of NRL for providing the DOD Plane Wave Code and Dr.Mehl of
NRL for providing the NRL TightBinding Code.Su Hao is also grateful for the discussions with Prof.
Freeman and Dr.Shishido of Northwestern University,and with Ms.Hsieh and Dr.Sherman of Cater
pillar Inc.
Fig.23.Toughness–strengthadhesion (TSA) diagram for steel design:(a) interfacial traction–separation relations with various dec
ohesion energy and (b) TSA diagram where CODi refers the COD at crack initiation.
1900 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
Appendix A.Preliminary of quantum mechanics and density functional theory [5,6,8,12]
Classical physics views an atom as a nuclei at ﬁxed point surrounded by moving electrons along ﬁxed
orbits.The momentums and positions of nuclei and electrons can be determined exactly according to
Newtons laws.
Quantum mechanics explains nature phenomena through another philosophy.The De Broglie
hypothesis ascribes a wave property to particles such as nuclei and electrons.The Heisenberg uncertainty
principle puts forth that,when the momentumof a particle is known precisely,the position of the particle is
completely unknown.The state of such a particle is deﬁned by Hamiltonian
b
H,the operator corresponding
to the energy of a particle with mass m
b
H ¼
h
2
2m
r
2
þV ðrÞ;ðA:1Þ
where r is the position vector and V ðrÞ is a potential ﬁeld.The eigenvalue equation for
b
H:
b
Hu
i
ðrÞ ¼ E
i
u
i
ðrÞ ðA:2Þ
is called the timeindependent Schr
€
odingers equation;where E
i
is the ith eigenvalue and u
i
ðrÞ the ith
eigenfunction.Under this state the expectation to ﬁnd the particle at position x is
hxi ¼
Z
1
1
ru
i
ðrÞ u
i
ðrÞd
3
r ¼
Z
1
1
rju
i
ðrÞj
2
d
3
r:ðA:3Þ
For a many body system,it is usually very diﬃcult to get analytical solution of (A.2) because the po
tential V ðrÞ is dependent of the interaction among particles.
Thomas–Fermi model approximates the systemas a combination of static atoms which formcrystal and
electronic gas which is ﬁlled inbetween.The Hohenberg–Kohn [5] and Kohn–Sham [6] theory states that
the total energy E
total
of a system depends only on the electron density of its ground state
E
total
¼ E
total
ðqðrÞ;R
a
Þ;ðA:4Þ
where R
a
are the position of all atoms in the system under consideration;the electron density q is a scale
function deﬁned as
qðrÞ ¼
X
i
ju
i
ðrÞj
2
:ðA:5Þ
The Hohenberg–Kohn–Sham theorem,the central theorem of the density functional theory,states that
the total system energy gets its minimum value for the groundstate density,denoted as q
0
,and that the
total energy is stationary with respect to its ﬁrst order variations in the density,i.e.:
dE
total
½q
dq
q¼q
0
¼ 0:ðA:6Þ
By varying E
total
with respect to each wave function,it leads to the Kohn–Shams equation:
Hw
i
ðrÞ ¼ e
i
w
i
ðrÞ;H ¼
h
2
2m
r
2
þV
eff
ðrÞ;ðA:7Þ
where w
i
ðrÞ,the solution of Kohn–Shams equation,form an orthonormal set;and the eﬀective potential is
V
eff
ðrÞ ¼ V
C
ðrÞ þl
XC
ðqÞ:ðA:8Þ
Here V
C
ðrÞ is the Coulomb potential;for a condensed system like metal V
C
ðrÞ can be solved through
Poissons equation
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1901
r
2
V
C
ðrÞ ¼ 4pe
2
qðrÞ;ðA:9Þ
where the qðrÞ denotes the positive point charges of nuclei at its position R
a
and the electronic charge
density qðrÞ in the rest
qðrÞ ¼
Z
r
at R
a
;
qðrÞ otherwise:
The exchangecorrelation potential l
XC
ðqÞ is related to the exchangecorrelation energy that can not
solved directly in the same way as V
C
ðrÞ.Under the ‘‘local density approximation’’ (LDA) the explicit form
of l
XC
ðqÞ has been derived,e.g.in [103,104]
l
XC
ðqÞ ¼ 2
3q
p
1=3
0:0225Log 1
þ21
4pq
3
1=3
!
:ðA:10Þ
One way to solve (A.7) is to expand the unknown wave function solutions w
i
ðrÞ as a linear combination
of a set of known function with unknown coeﬃcients c
ij
w
i
ðrÞ ¼
X
j
c
ij
/
i
ðrÞ:ðA:11Þ
Substituting (A.11) into (A.7) leads to the following matrix problem:
½
HS c ¼ 0;ðA:12Þ
where
H is the Hamiltonian matrix and S is the overlap matrix
½
H
ij
¼
Z
/
i
H /
j
dr;½S
ij
¼
Z
/
i
/
j
dr ðA:12aÞ
in the ﬁrst relation of (A.12a) the H is deﬁned by (A.7).
The solution procedure is illustrated in Fig.24.
In a periodic structure such as a crystal,according to Bloch theorem the wave function solution w
i
depends upon both position vector r and the reciprocal vector k
w
i
ðr þmG;kÞ ¼ e
ikG
w
i
ðr;kÞ;ðA:13Þ
where G is the primitive vector of the lattice and m is an integer.The corresponding electron density yields
the integration over the ﬁrst Brillouin zone:
qðrÞ ¼
Z
1
st
BZ
#½E
F
e
i
ðkÞjw
i
ðr;kÞj
2
dk;ðA:14Þ
where the step function#insures that only occupied states below the Fermi energy E
F
are counted.
Appendix B.Corotational formulation in ﬁnite deformation
The corotational formulation introduced in [60,105] is applied in the analysis presented in this work.We
use boldfaced x to represent the coordinate of a material point in a reference coordinate system,i.e.the
Lagrange conﬁguration;and boldfaced y to represents the coordinate of a point in the spatial (Euler)
coordinate system.Obviously
y ¼ yðx;tÞ:ðB:1Þ
1902 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
Consider a line element vector dr
0
in the reference conﬁguration,after deformation it becomes the line
element dr in the spatial conﬁguration.The deformation gradient is deﬁned by
Fðx;tÞ ¼
oy
ox
;ðB:2Þ
which uniquely determines the line element transformation between the two conﬁgurations
dr ¼ Fdr
0
:ðB:3Þ
Using this relation we can also derive the transformation an area or a volume between two conﬁgura
tions.When we assume ﬁnite deformation without diﬀusion,then F is nonsingular and can be decomposed
multiplicatively as the product of two other positive deﬁnite tensors
F ¼ R
F
U
F
;ðB:4Þ
where R
F
is the orthogonal,positive deﬁnite,tensor of pure rotation from conﬁguration x to y;U
F
is the
positive deﬁnite tensor of pure stretch during deformation.The discussions of the transformations (B.1)–
(B.4) in crystal plasticity and atomistic simulation can be found in [106–108].
The material derivative of Eq.(B.2) leads to
_
Fðx;tÞ ¼
o
_
y
oy
oy
ox
¼ L F with L¼
def
o
_
y
oy
¼ rv:ðB:5Þ
Here we adopt r to represent the gradient operator in the spatial conﬁguration and v ¼
_
y,i.e.the velocity.
So L is called the ‘‘velocity gradient’’.L and Cauchy stress r build a conjugate energy pair.In general,the
rate constitutive relation of a material can be written as
_
r ¼ C:L þS:L
skew
;ðB:6Þ
where C is a material tangent matrix and L
skew
represents the skewsymmetric part of L.The product
S L
skew
reﬂects the change of stress state due to rigid rotations,therefore Eq.(B.6) is ‘‘nonobjective’’.
Fig.24.Flow chart of the solution procedure of DFT.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1903
In numerical analysis,when a body deforms from step n to step n þ1,its spatial coordinate y
nþ1
may be
written as a function of the conﬁguration at step n and the step length Dt
y
nþ1
¼ y
nþ1
ðy
n
;DtÞ ðB:7Þ
The displacement increment of this point over the step is
Du ¼ y
nþ1
y
n
:ðB:8Þ
An incremental form of the velocity gradient deﬁned in Eq.(B.5) is
L ¼
1
Dt
oDu
oy
nþ1
:ðB:9Þ
The key idea of the corotational formulation is to split one increment into two steps,i.e.rotation and
pure deformation.Consider the conﬁguration at y
n
as the reference conﬁguration
_
Fðy
n
;tÞ ¼
_
F
def
ðy
n
;tÞ
_
F
rot
ðy
n
;tÞ:ðB:10Þ
From Eq.(B.4) it is known that
_
F
rot
ðy
n
;tÞ ¼ R I and
_
F
def
ðy
n
;tÞ ¼
oy
nþ1
oy
n
L
def
¼ I
þ
oDu
def
oy
n
oDu
def
Dtoy
nþ1
;ðB:11Þ
where R deﬁnes the rotation from conﬁguration y
n
to y
nþ1
and I represents the unit tensor.If Du
def
is small
enough,then the second relation in Eqs.(B.11) becomes
_
F
def
ðy
n
;tÞ ¼ I L
def
þoðL
def
Þ:ðB:12Þ
The corresponding algorithm for integrating the constitutive equation is as follows:
^
r
nþ1
¼ R
T
r
n
R;
Dr ¼ C:ðDtL
def
Þ;
r
nþ1
¼
^
r
nþ1
þDr:
ðB:13Þ
The second relation in Eqs.(B.13) is ‘‘objective’’ since there is no rotation.
A concise way to calculate R is given in [105] when the rotation is less than p during Dt.Consider a mid
deformation conﬁguration:
y
nþa
¼ ð1 aÞy
nþ1
þay
n
with 0 < a < 1 ðB:14Þ
it has been proven,elsewhere,that
R ¼ 1
þ
1
2
x
1
1
2
x
1
;g ¼
oDu
oy
nþa
;x ¼
1
2
ðg g
T
Þ;ðB:15Þ
where I is unit tensor.a ¼ 0:5 is used in the analysis.
The formulation listed above can be applied in both Lagrange conﬁgurationbased and Euler conﬁgu
rationbased computation.When a Lagrange conﬁguration is applied,the corresponding derivative oper
ations are derived in the reference conﬁguration x while the velocity is deﬁned with respect to the current
conﬁguration y
nþ1
,a transformation matrix J is necessary for deﬁning the large strainvelocity matrix
e
B.
o
oy
nþ1
¼
o
ox
ox
oy
nþ1
¼
o
ox
J:ðB:16Þ
Because of
ox
ox
¼
ox
oy
nþ1
oy
nþ1
ox
¼ I:ðB:17Þ
1904 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
Thus,we have
J ¼
oy
nþ1
ox
1
:ðB:18Þ
Appendix C.The approximation of additive decomposition (5.1)
In a corotation coordinate system introduced in Appendix B,the rotation part is removed and the
deformation can be divided into two steps:pure elastic transformation F
e
and plastic transformation F
p
[109]
F ¼ F
p
F
e
Following the procedure giving in [60],the velocity gradient L of the deformation ﬁeld (B.1),deﬁned as
the mass derivative of F,is
L ¼
DF
Dt
¼
oF
ot
F
1
¼
_
F F
1
;ðC:1Þ
which has two parts
_
F F
1
¼
_
F
e
F
p
ðF
e
F
p
Þ
1
þF
e
_
F
p
ðF
e
F
p
Þ
1
¼
_
F
e
ðF
e
Þ
1
þF
e
_
F
p
ðF
p
Þ
1
ðF
e
Þ
1
ðC:2Þ
In this paper,we assume that elastic deformation is inﬁnitesimal so that
F
e
¼ I þ
ou
e
ox
¼ I þoðIÞ;ðF
e
Þ
1
¼ I oðIÞ
and
L ¼
_
F F
1
ﬃ
_
F
e
ðF
e
Þ
1
þ
_
F
p
ðF
p
Þ
1
Deﬁne strain rate as the symmetrical part of the velocity gradient
_
¼ symðLÞ:
We obtain the additive decomposition of strain rate
_
:
_
¼
_
e
þ
_
p
;ð5:1Þ
where
_
e
¼ symð
_
F
e
ðF
e
Þ
1
Þ;
_
p
¼ symð
_
F
p
ðF
p
Þ
1
Þ:
References
[1] Cybersteel2020,ONR contract grant number:N000140110953;PIs:Olson GB,Freeman A,Liu WK,Moran B,Northwestern
University.
[2] J.R.Rice,Dislocation nucleation from a crack tip––an analysis based on the Peierls concept,J.Mech.Phys.Solids 40 (2) (1992)
239–271.
[3] L.H.Thomas,The calculation of atomic ﬁelds,Proc.Camb.Philos.Soc.23 (1927) 542–548.
[4] E.Fermi,A statistical method for the determination of some atomic properties and the application of this method to the theory
of the periodic system of elements,Z.Phys.48 (1928) 73–79.
[5] P.Hohenberg,W.Kohn,Inhomogeneous electron gas,Phys.Rev.136 (3B) (1964) 864–871.
[6] W.Kohn,L.J.Sham,Selfconsistent equations including exchange and correlation eﬀects,Phys.Rev.140 (4A) (1965) 1133–1138.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1905
[7] J.C.Slater,Wave functions in a periodic potential,Phys.Rev.51 (1937) 846–851.
[8] H.Krakauer,A.J.Freeman,Linearized augmented planewave method for the electronic bandstructure of thinﬁlms,Phys.Rev.
B 19 (4) (1979) 1706–1719.
[9] NRL,DoD plane wave:a general scalable density functional code,2002.
[10] M.J.Mehl,D.A.Papaconstantopoulos,Applications of a tightbinding totalenergy method for transition and noble metals:
elastic constants,vacancies,and surfaces of monatomic metals,Phys.Rev.B 54 (7) (1996) 4519–4530.
[11] D.A.Papaconstantopoulos,M.J.Mehl,The tightbinding method for interpolating ﬁrstprinciples total energy results,J.Phase
Equilib.18 (6) (1997) 593–597.
[12] E.Wimmer et al.,Fullpotential selfconsistent linearizedaugmentedplanewave method for calculating the electronicstructure
of molecules and surfaces––O
2
molecule,Phys.Rev.B 24 (2) (1981) 864–875.
[13] J.H.Rose,J.R.Smith,J.Ferrante,Universal features of bonding in metals,Phys.Rev.B 28 (4) (1983) 1835–1845.
[14] J.Weertman,Crack tip blunting by dislocation pair creation and separation,Philos.Mag.A––Phys.Cond.Matter Struct.
Defects Mech.Prop.43 (5) (1981) 1103–1123.
[15] S.H.Jhi,J.Ihm,S.G.Louie,M.L.Cohen,Electronic mechanism of hardness enhancement in transitionmetal carbonitrides,
Nature 399 (6732) (1999) 132–134.
[16] T.Shishidou et al.,Overlayer and superlattice studies of metal/ceramic interfaces:Fe/TiC,J.Appl.Phys.93 (10) (2003) 6876–
6878.
[17] T.Shishidou,Y.J.Zhao,A.J.Freeman,private discussion,2002.
[18] M.J.S.Spencer et al.,Further studies of iron adhesion:(11 1) surface,Surf.Sci.515 (2002) L464–468.
[19] M.J.Mehl,A.Papaconstantopoulos,Application of a tightbinding totalenergy method for transition and noble metals:elastic
constants,vacancies,and surfaces of monatomic metals,Phys.Rev.B 54 (7) (1996) 4519–4530.
[20] S.H.Jhi,J.Ihm,Electronic structure and structural stability of TiC
x
N
1x
alloys,Phys.Rev.B 56 (21) (1997) 13826–13829.
[21] A.J.Freeman,Materials by design and the exciting role of quantum computation/simulation,J.Computat.Appl.Math.149 (1)
(2002) 27–56.
[22] D.G.Pettifor,A.H.Cottrell (Eds.),Electron Theory in Alloy Design,The Institute of Materials,London,1992.
[23] A.Needleman,A continuum model for void nucleation by inclusion debonding,J.Appl.Mech.,ASME,Trans.54 (3) (1987)
525–531.
[24] A.S.Argon,J.Im,R.Safoglu,Cavity formation from inclusions in ductile fracture,Metal.Trans.A6 (4) (1975) 825–837.
[25] J.A.Hurtado,B.R.Elliott,H.M.Shodja,D.V.Gorelikov,C.E.Campbell,H.E.Lippard,T.C.Isabell,J.Weertman,Disclination
grainboundary model with plasticdeformation by dislocations,Mater.Sci.Engrg.A––Struct.Mater.Propert.Microstruct.
Process.190 (1–2) (1995) 1–7.
[26] J.R.Rice,in:A.W.Thompson,I.M.Bernstein (Eds.),Eﬀect of Hydrogen on Behavior of Materials,The Metallurgical Society of
AIME,Warrendale,PA,1976,p.455.
[27] J.R.Rice,J.S.Wang,Embrittlement of interfaces by solute segregation,Mater.Sci.Engrg.A––Struct.Mater.Propert.
Microstruct.Process.107 (1989) 23–40.
[28] J.P.Hirth,J.R.Rice,On the thermodynamics of adsorption at interfaces as it inﬂuences decohesion,Metal.Trans.A––Phys.
Metal.Mater.Sci.11 (9) (1980) 1501–1511.
[29] R.J.Asaro,Adsorptioninduced losses in interfacial cohesion,Philos.Trans.R.Soc.London Ser.A––Math.Phys.Engrg.Sci.
295 (1413) (1980) 151–163.
[30] I.Alber,J.L.Bassani,M.Khantha,V.Vitek,G.J.Wang,Grain boundaries as heterogeneous system atomic and continuum
elastic properties,Philos.Trans.R.Soc.London A 339 (1992) 555–586.
[31] S.Hao,W.K.Liu,B.Moran,Particle dynamics (in preparation).
[32] M.S.Daw,M.I.Baskes,Embeddedatom method––derivation and application to impurities,surfaces,and other defects in
metals,Phys.Rev.B 29 (12) (1984) 6443–6453.
[33] M.I.Baskes,Embedded atom method atomistic calculations of the dynamic interaction of an edge dislocation in nickel with
helium clusters,J.Metals 40 (11) (1988) 123.
[34] W.K.Liu,S.Jun,Y.F.Zhang,Reproducing Kernel particle methods,Int.J.Numer.Methods Fluids 20 (1995) 1081–1106.
[35] T.Belytschko,Y.Y.Lu,L.Gu,Elementfree Galerkin methods,Int.J.Numer.Methods Engrg.37 (1994) 229–256.
[36] W.K.Liu,S.Jun,S.Li,J.Adee,T.Belytschko,Reproducing Kernel particle methods for structural dynamics,Int.J.Numer.
Methods Engrg.38 (1995) 1655–1680.
[37] J.T.Oden,K.Vemaganti,Adaptive hierarchical modeling of heterogeneous structures,Physica D 133 (1–4) (1999) 404–415.
[38] T.J.R.Hughes,Multiscale phenomena––Greensfunctions,the DirichlettoNeumann formulation,subgrid scale models,bubbles
and the origins of stabilized methods,Comput.Methods Appl.Mech.Engrg.127 (1–4) (1995) 387–401.
[39] J.S.Chen,S.P.Yoon,C.T.Wu,Nonlinear version of stabilized conforming nodal integration for Galerkin meshfree methods,
Int.J.Numer.Methods Engrg.53 (12) (2002) 2587–2615.
[40] W.K.Liu,R.A.Uras,Y.Chen,Enrichment of the ﬁnite element method with the reproducing Kernel particle method,J.Appl.
Mech.,ASME 64 (1997) 861–870.
1906 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
[41] W.K.Liu,Y.F.Zhang,M.R.Ramirez,Multiple scale ﬁnite element methods,Int.J.Numer.Methods Engrg.32 (1991) 960–990.
[42] L.Ghosh,K.Lee,P.Raghavan,A multilevel computational model for multiscale damage analysis in composite and porous
materials,Int.J.Solids Struct.38 (14) (2001) 2335–2385.
[43] S.Hao,H.S.Park,W.K.Liu,Moving particle ﬁnite element method,In.J.Numer.Methods Engrg.53 (8) (2002) 1937–
1958.
[44] G.J.Wagner,W.K.Liu,Coupling of atomistic and continuum simulations using a bridging scale decomposition,J.Computat.
Phys.(accepted).
[45] L.E.Shilkrot,W.A.Curtin,R.E.Miller,A coupledatomistic/continuum model of defects in solids,J.Mech.Phys.Solids 50 (10)
(2002) 2085–2162.
[46] T.Belytschko,Y.Krongauz,D.Organ,M.Fleming,P.Krysl,Meshless methods:An overview and recent developments,
Comput.Methods Appl.Mech.Engrg.139 (1–4) (1996) 3–47.
[47] S.F.Li,W.K.Liu,Meshfree and particle methods and their applications,Appl.Mech.Rev.55 (2002) 1–34.
[48] T.P.Fries,H.G.Matthies,Classiﬁcation and overview of meshfree methods,Tech.University of Braunschweig,Brunswick,
Germany,March 2003.
[49] D.J.Oh,R.A.Johnson,Simple embedded atom method model for Fcc and Hcp metals,J.Mater.Res.3 (3) (1988) 471–478.
[50] J.H.Rose,J.R.Smith,F.Guinea,J.Ferrante,Universal features of the equation of state of metals,Phys.Rev.B 29 (6) (2002)
2963–2969.
[51] R.A.Johnson,D.J.Oh,Analytic embedded atom method model for Bcc metals,J.Mater.Res.4 (5) (1989) 1195–1201.
[52] M.F.Horstemeyer et al.,A multiscale analysis of ﬁxedend simple shear using molecular dynamics,crystal plasticity,and a
macroscopic internal state variable theory,Model.Simulat.Mater.Sci.Engrg.11 (3) (2003) 265–286.
[53] N.W.Ashcroft,N.D.Mermin,Solid State Physics,Saunders College Publishing,1976.
[54] E.B.Tadmor,M.Ortiz,R.Phillips,Quasicontinuum analysis of defects in solids,Philos.Mag.A––Phys.Cond.Matter Struct.
Defects Mech.Propert.73 (6) (1996) 1529–1563.
[55] M.Ortiz et al.,Mixed atomistic continuum models of material behavior:The art of transcending atomistics and informing
continua,MRS Bull.26 (3) (2001) 216–221.
[56] S.Hao,W.K.Liu,D.Qian,Localizationinduced band and cohesive model,J.Appl.Mech.––Trans.ASME 67 (4) (2000) 803–
812.
[57] H.S.Park,W.K.Liu,An introduction and tutorial on multiple scale analysis in solids,Computat.Methods Appl.Mech.Engrg.
(accepted).
[58] D.Qian,J.Wagner,W.K.Liu,Amultiscale projection method for the analysis of carbon nanotubes,Computat.Methods Appl.
Mech.Engrg.(accepted).
[59] W.K.Liu,K.,E.G.,Zhang,S.,Park,H.S.,An introduction to computational nanomechanics and materials,Comput.Methods
Appl.Mech.Engrg.(2003) (accepted).
[60] T.Belytschko,W.K.Liu,B.Moran,Nonlinear Finite Elements for Continua and Structures,John Wiley,Chichester New York,
2000,xvi,650.
[61] P.Zhang et al.,The elastic modulus of singlewall carbonnanotubes:a continuum analysis incorporating interatomic potentials,
Int.J.Solids Struct.39 (1314) (2002) 3893–3906.
[62] G.B.Olson,K.C.Hsieh,Technical Report,Department of Mater Science Engineering,Northwestern University,2002.
[63] C.L.Briant,et al.,Void nucleation in a low alloy steel,in:TMS Meeting.2002.
[64] J.D.Eshelby,Elastic inclusions and inhomogeneities,in:I.N.Sneddon,R.Hill (Eds.),Progress in Solid Mechanics,North
Holland,Amsterdam,1961,pp.89–140.
[65] R.Hill,Continuum micromechanics of elastoplastic polycrystals,J.Mech.Phys.Solids 13 (1965) 89–101.
[66] J.W.Hutchinson,Elastic–plastic behaviour of polycrystalline metals and composites,Proc.R.Soc.London Ser.A––Math.Phys.
Sci.319 (1537) (1970) 247.
[67] J.R.Rice,D.M.Tracey,On the ductile enlargement of voids in triaxial stress ﬁeld,J.Mech.Phys.Solids 17 (1969) 2–15.
[68] A.L.Gurson,Continuum theory of ductile rupture by void nucleation and growth:Part I––Yield criteria and ﬂow rules for
porous ductile media,J.Engrg.Mater.Technol.99 (1977) 2–15.
[69] V.Tvargaard,J.W.Hutchinson,On localization in ductile materials containing spherical voids,Int.J.Fract.18 (1982) 237–252.
[70] S.Socrate,D.M.Parks,1995,MIT,Cambridge.
[71] A.S.Khan,Y.Parikh,Astudy of 2 incremental theories of plasticity through large deformation in polycrystalline copper,Engrg.
Fract.Mech.21 (4) (1985) 697–707.
[72] B.Moran,R.J.Asaro,C.F.Shih,Eﬀects of material rate sensitivity and void nucleation on fracture initiation in a
circumferentially cracked bar,Met.Trans.22A (1991) 161–170.
[73] J.D.Embury,Damage and failure processes in structuralmaterials,J.Phys.IV 3 (C7) (1993) 607–619.
[74] J.M.Duva,Hutchinson,Constitutive potentials for dilutely voided nonlinear materials,J.Mech.Mater.3 (1984) 41–54.
[75] A.G.Evans,M.C.Lu,S.Schmauder,M.Ruhle,Some aspects of the mechanical strength of ceramic metal bonded systems,Acta
Metal.Mater.34 (8) (1986) 1634–1655.
S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1907
[76] J.Fan,A micro/macroscopic analysis for cyclic plasticity of dualphase materials,J.Appl.Mech.66 (1999) 124–130.
[77] P.Ladeveze,A damage computational method for composite structures,Comput.Struct.44 (12) (1992) 79–87.
[78] A.S.Khan,P.Cheng,An anisotropic elastic–plastic constitutive model for single and polycrystalline metals.II––Experiments
and predictions concerning thinwalled tubular OFHC copper,Int.J.Plast.14 (1–3) (1998) 209–226.
[79] D.L.McDowell et al.,Micro structurebased fatigue modeling of cast A356T6 alloy,Engrg.Fract.Mech.70 (1) (2003) 49–80.
[80] P.G.Sanders,C.J.Youngdahl,J.R.Weertman,The strength of nanocrystalline metals with and without ﬂaws,Mater.Sci.Engrg.
A––Struct.Mater.Propert.Microstruct.Process.234 (1997) 77–82.
[81] T.J.R.Hughes,L.P.Franca,M.Mallet,A new ﬁniteelement formulation for computational ﬂuiddynamics.1.Symmetrical
forms of the compressible Euler and NavierStokes equations and the 2nd law of thermodynamics,Comput.Methods Appl.
Mech.Engrg.54 (2) (1986) 223–234.
[82] P.Germain,Q.S.Nguyen,P.Suquet,Continuum thermodynamics,J.Appl.Mech.,ASME Trans.50 (4B) (1983) 1010–1020.
[83] J.L.Chaboche,Constitutiveequations for cyclic plasticity and cyclic viscoplasticity,Int.J.Plast.5 (3) (1989) 247–302.
[84] M.F.Horstemeyer,P.Wang,Cradletograve simulationbased design incorporating multiscale microstructureproperty
modeling:Reinvigorating design with science,J.Comput.Aided Mater.Design (in press).
[85] S.Hao,W.K.Liu,C.T.Chang,Computer implementation of damage models by ﬁnite element and meshfree methods,Comput.
Methods Appl.Mech.Engrg.187 (3–4) (2000) 401–440.
[86] J.F.Bishop,R.Hill,A theory of the plastic distortion of polycrystalline aggregate under combined stresses,Philos.Mag.42
(1951) 414–427.
[87] P.Klein,H.J.Gao,Crack nucleation and growth as strain localization in a virtualbond continuum,Engrg.Fract.Mech.61
(1998) 21–48.
[88] S.Hao,W.K.Liu,P.Klein,Multiscale damage model 2000,Chicago,IL,USA,IUTAM2000.
[89] V.Tvargaard,J.W.Hutchinson,Inﬂuence of voids on shear band instabilities under plane strain condition,Int.J.Fract.Mech.
17 (1981) 389–407.
[90] S.Hao,W.K.Liu,A.Rosakis,P.Klein,Modeling and Simulation of Intersonic Crack Growth,Northwestern University,M.
Engineering,2001.
[91] N.A.Fleck,G.M.Muller,M.F.Ashby,J.W.Hutchinson,Strain gradient plasticity:theory and experiment,Acta Metal.Mater.
42 (1994) 475–487.
[92] H.Gao,Y.Huang,W.D.Nix,J.W.Hutchinson,Mechanismbased strain gradient plasticity––I.Theory,J.Mech.Phys.Solids 47
(6) (1999) 1239–1263.
[93] V.Tvergaard,A.Needleman,Eﬀect of crack meandering on dynamic,ductile fracture,J.Mech.Phys.Solids 40 (2) (1992) 447–
471.
[95] S.Hao,W.Brocks,The Gurson–Tvergaard–Needlemanmodel for rate and temperaturedependent materials with isotropic and
kinematic hardening,Computat.Mech.20 (1–2) (1997) 34–40.
[96] S.Hao,W.K.Liu,Moving particle ﬁnite element method with global superconvergence (submitted).
[97] B.Moran,F.Shih,Crack tip and associated domain integrals from momentum and energybalance,Engrg.Fract.Mech.27 (6)
(1987) 615–642.
[98] B.Moran,F.Shih,A general treatment of crack tip contour integrals,Int.J.Fract.35 (4) (1987) 295–310.
[99] P.G.Mcdougall,G.B.Olson,M.Cohen,Interphase crystallography and interfacial structure,J.Metals 35 (12) (1983) 17.
[100] J.D.Landes,K.Brown,Results from a round robin on a standard method for measurement of fracture toughness,J.Testing
Evaluat.26 (4) (1998) 396–403.
[101] K.H.Schwalbe,Inﬂuence of microstructure on crackpropagation mechanisms and fracture toughness of metallic materials,
Engrg.Fract.Mech.9 (4) (1977) 795–832.
[102] A.Saxena,Creep crackgrowth in hightemperature ductile materials,Engrg.Fract.Mech.40 (4–5) (1991) 721–736.
[103] R.Gaspar,Acta Phys.Acad.Sci.Hung.3 (1954) 263.
[104] L.Heidin,S.J.Lundqvist,Phys.(France) 33 (C373) (1972).
[105] T.J.R.Hughes,J.Winget,Finite rotation eﬀects in numerical integration of rate constitutive equations arising in large
deformation analysis,Int.J.Numer.Methods Engrg.15 (1980) 1862–1867.
[106] M.F.Horstemeyer,M.I.Baskes,Atomistic ﬁnite deformation simulations:a discussion on length scale eﬀects in relation to
mechanical stresses,J.Engrg.Mater.Technol.––Trans.ASME 121 (2) (1999) 114–119.
[107] A.S.Khan,X.M.Su,Constitutive relations for singlecrystal based on 2 surface description,Int.J.Plast.10 (7) (1994) 807–823.
[108] A.S.Khan,Y.Parikh,Large deformation in polycrystalline copper under combined tension–torsion,loading,unloading and
reloading or reverse loading––a study of 2 incremental theories of plasticity,Int.J.Plast.2 (4) (1986) 379–392.
[109] E.H.Lee,Elastic–plastic deformation at ﬁnite strain,J.Appl.Mech.36 (1969) 1–6.
1908 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908
Enter the password to open this PDF file:
File name:

File size:

Title:

Author:

Subject:

Keywords:

Creation Date:

Modification Date:

Creator:

PDF Producer:

PDF Version:

Page Count:

Preparing document for printing…
0%
Σχόλια 0
Συνδεθείτε για να κοινοποιήσετε σχόλιο